@A340-500/600

SERVICE BULLETIN

REVISION TRANSMITTAL SHEET

AIRBUS

CUSTOMER SERVICES DIRECTORATE

1 Rond Point Maurice Bellonte

31707 BLAGNAC CEDEX

FRANCE

Tel : (33) 5 61 93 33 33

Telex : AIRBU 530526F

Fax : (33) 5 61 93 42 51

MANDATORY MANDATORY MANDATORY

ATA SYSTEM: 55

TITLE: STABILIZERS - RUDDER SIDE SHELL SANDWICH REPAIR

INSPECTION

MODIFICATION No.: None

This page transmits Revision No.01 of Service Bulletin No.A340-55-5007

ADDITIONAL WORK

**CONF ALL

No additional work is required by this revision for aircraft modified by any previous issue.

REASON

Revision No. 01 issued to embody the local sanding procedure.

CHANGES

SUMMARY

EFFECTIVITY OPERATOR LIST UPDATED R

REFERENCES / REPERCUSSIONS REFERENCES/REPERCUSSIONS TABLE

UPDATED

R

PLANNING INFORMATION

EFFECTIVITY EFFECTIVITY RELATED INFORMATION

UPDATED

R

COMPLIANCE

Accomplishment Timescale ACCOMPLISHMENT TIMESCALE UPDATED R

MANPOWER MANPOWER UPDATED R

REFERENCES REFERENCED DOCUMENTATION UPDATED R

MATERIAL INFORMATION

LIST OF MATERIALS - OPERATOR

SUPPLIED

Consumable Materials

Consumable CMLD01 CONSUMABLE MATERIAL SET UPDATED

CONSUMABLE UPDATED

R

TOOLING

Tools TOOLS UPDATED R

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 1

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

REVISION TRANSMITTAL SHEET

ACCOMPLISHMENT INSTRUCTIONS

TASK 555007- 832-848-001-Inspection TASK SOLUTION UPDATED

NOTE UPDATED

R

Subtask 555007-910-201-001 SUBTASK SOLUTION UPDATED

QUANTITY UPDATED

CONSUMABLE UPDATED

MATERIAL LIST UPDATED

R

Subtask 555007-941-201-001 SUBTASK SOLUTION UPDATED

NOTE UPDATED

R

Subtask 555007-832-201-001 SUBTASK SOLUTION UPDATED

FIGURE REFERENCE UPDATED

R

Subtask 555007-832-202-001 SUBTASK SOLUTION UPDATED

QUANTITY UPDATED

CONSUMABLE UPDATED

MATERIAL LIST UPDATED

FIGURE REFERENCE UPDATED

NOTE UPDATED

R

Subtask 555007-832-203-001 SUBTASK SOLUTION UPDATED

QUANTITY UPDATED

CONSUMABLE UPDATED

MATERIAL LIST UPDATED

FIGURE REFERENCE UPDATED

NOTE UPDATED

R

Subtask 555007-832-204-001 SUBTASK SOLUTION UPDATED

CONSUMABLE UPDATED

FIGURE REFERENCE UPDATED

NOTE UPDATED

CONFIGURATION UPDATED

MATERIAL LIST UPDATED

R

Subtask 555007-832-205-001 SUBTASK SOLUTION UPDATED

QUANTITY UPDATED

CONSUMABLE UPDATED

MATERIAL LIST UPDATED

REFERENCED DOCUMENTATION UPDATED

FIGURE REFERENCE UPDATED

REFERENCES UPDATED

R

Subtask 555007-832-206-001 SUBTASK SOLUTION UPDATED

CONSUMABLE UPDATED

FIGURE REFERENCE UPDATED

NOTE UPDATED

MATERIAL LIST UPDATED

R

Subtask 555007-832-207-001 SUBTASK SOLUTION UPDATED

QUANTITY UPDATED

CONSUMABLE UPDATED

MATERIAL LIST UPDATED

NOTE UPDATED

R

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 2

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

REVISION TRANSMITTAL SHEET

Subtask 555007-833-201-001 SUBTASK SOLUTION UPDATED

QUANTITY UPDATED

CONSUMABLE UPDATED

REFERENCED DOCUMENTATION UPDATED

MATERIAL LIST UPDATED

R

Subtask 555007-832-208-001 SUBTASK SOLUTION ADDED N

Subtask 555007-942-201-001 SUBTASK SOLUTION UPDATED R

Fig. A-GBFAA

Fig. A-GBFAA Sheet 02 SHEET UPDATED R

Fig. A-GBHAA FIGURE SOLUTION UPDATED R

Fig. A-GBHAA Sheet 01 SHEET UPDATED R

Fig. A-GBHAA Sheet 02 SHEET UPDATED R

Fig. A-GBHAA Sheet 03 SHEET UPDATED R

Fig. A-GBHAA Sheet 04 SHEET ADDED N

Fig. A-GFAAA FIGURE SOLUTION UPDATED R

Fig. A-GFAAA Sheet 01 SHEET UPDATED R

Fig. A-GFAAA Sheet 02 SHEET UPDATED R

Fig. A-GFAAA Sheet 03 SHEET UPDATED R

Fig. A-GFAAA Sheet 04 SHEET UPDATED R

Fig. A-GFAAA Sheet 05 SHEET UPDATED R

Fig. A-GFAAA Sheet 06 SHEET ADDED N

Fig. A-GAAAA

Fig. A-GAAAA Sheet 01 SHEET UPDATED R

Fig. A-GABAA

Fig. A-GABAA Sheet 04 SHEET UPDATED R

Fig. A-GABAA Sheet 08 SHEET UPDATED R

FILLING INSTRUCTIONS

This Service Bulletin has been generated electronically and is reissued as a complete document.

Replace the complete document.

Put this Revision Transmittal Sheet in front of the Service Bulletin.

HISTORY OF PREVIOUS REVISIONS

No previous revision

REVISION SEQUENCE

ORIGINAL: Feb 07/13

REVISION No. : 01 - Aug 20/14

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 3

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

REVISION TRANSMITTAL SHEET

This Page Intentionally Left Blank

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 4

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

SUMMARY

AIRBUS

CUSTOMER SERVICES DIRECTORATE

1 Rond Point Maurice Bellonte

31707 BLAGNAC CEDEX

FRANCE

Tel : (33) 5 61 93 33 33

Telex : AIRBU 530526F

Fax : (33) 5 61 93 42 51

This summary is for information only and is not approved for modification of the aircraft.

MANDATORY MANDATORY MANDATORY

ATA SYSTEM: 55

TITLE: STABILIZERS - RUDDER SIDE SHELL SANDWICH REPAIR

INSPECTION

**CONF ALL

MODIFICATIONS

None

REASON/DESCRIPTION/OPERATIONAL CONSEQUENCES

On AIRBUS Single Aisle, Long Range and Wide Body family aircraft, the rudder side shell is a

sandwich structure made of Carbon Fiber Reinforced Plastic (CFRP) and Glass Fiber Reinforced Plastic

(GFRP) with a honeycomb core. A case of skin damage was reported on a composite side panel of a

rudder installed on an A310 aircraft. Investigations have shown that the damage started from a skin

panel area previously repaired in-service. This repair was performed as per A310 SRM 55-41-12 Fig.

204 procedure. The new damage has been identified as a damage between the core and the skin in

the repaired area. This new damage has developed during normal operations due to the variation of

pressure during ground-air-ground cycles.

Following the above mentioned damage scenario, it has been identified that SRM procedures need to

be improved to ensure an adequate repair quality. An improper bonding between skin and core during a

repair may lead to a damage initiation and propagation, which may not be detectable visually. A large

rudder damage, resulting from an undetected damage growth, could affect the handling quality of the

aircraft.

This Service Bulletin details the inspection procedure to inspect affected rudders fitted on A340 aircraft

for potential damage.

Different inspection procedures are necessary:

- Pulse thermography inspection

- Elasticity Laminate Checker (ELCH) inspection

- Ultrasonic Testing (UT) inspection.

- Tap test inspection.

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 1

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

SUMMARY

The accomplishment of this Service Bulletin will contribute to detect potential damage around in-service

repairs accomplished on rudders made of Carbon Fiber Reinforced Plastic (CFRP) and Glass Fiber

Reinforced Plastic (GFRP) with a honeycomb core.

GENERAL EVALUATION

EVALUATION TABLE

COMPLIANCE MANDATORY (1) CANCELS INSPECTION SB NO

POTENTIAL AD YES A/C OPERATION AFFECTED NO

RELIABILITY AFFECTED NO PAX COMFORT AFFECTED NO

COST SAVING NO LROPS AFFECTED NO

STRUCTURAL LIFE EXTN NO VENDOR SB INVOLVED NO

NOTE (1): Service Bulletin must be accomplished.

MATERIAL PRICE INFORMATION

No Material

EFFECTIVITY

This Service Bulletin is applicable to this (these) operator(s) :

06U 25R 36V 70U 72W AHY AIB CES CHH DLH ETD HFM HFY

IBE QAF QTR SAA SIA TAM THA UAE VIR

CONCURRENT REQUIREMENTS

None

REFERENCES / REPERCUSSIONS

TFU None

OEB None

AOT None

SIL None

LINE MAINTENANCE AFFECTED No

LIFE LIMIT None

OTHER OIT 999.0017/10 OIT 999.0071/10 OIT 999.0130/06 OIT

999.0067/12 AD 2014-0033

NATURE OF THE WORK

AIRCRAFT YES

EQUIPMENT NO

HARD NO

SOFT NO

OBRM NO

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 2

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

SUMMARY

MANPOWER

Task 555007-832-848-001: Inspection

TOTAL MANHOURS 38.00

APPENDICES

None

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 3

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

SUMMARY

**CONF ALL

Z326

A

RUDDER SHELL

TO BE INSPECTED

B

B A

RH SHOWN LH SHOWN

F_SB_555007_6_SAAA_01_01

Figure A-GSAAA - Sheet 01

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 4

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

AIRBUS

CUSTOMER SERVICES DIRECTORATE

1 Rond Point Maurice Bellonte

31707 BLAGNAC CEDEX

FRANCE

Tel : (33) 5 61 93 33 33

Telex : AIRBU 530526F

Fax : (33) 5 61 93 42 51

MANDATORY MANDATORY MANDATORY

ATA SYSTEM: 55

TITLE: STABILIZERS - RUDDER SIDE SHELL SANDWICH REPAIR

INSPECTION

MODIFICATION No.: None

This document contains AIRBUS PROPRIETARY INFORMATION and shall at all times remain the

property of AIRBUS; no intellectual property right or licence is granted by AIRBUS in connection with

any information contained in it. It is delivered on the express condition that said document and the

information contained in it shall be treated as confidential, shall not be used for any purpose other than

that for which it is hereby delivered. It shall not be disclosed in whole or in part to third parties and shall

not be duplicated in any manner (except for the purposes of performing the tasks described hereunder

and provided that any recipient of such document shall comply with the conditions herein), without

AIRBUS prior written consent.

1. PLANNING INFORMATION

**CONF ALL

A. EFFECTIVITY

NOTE: This Service Bulletin is applicable to all rudders with the Serial Number (SN)

from TS-5001 to TS-5138.

NOTE: The related SRM procedures do currently not exist for A340-500/600 aircraft,

but in case that repairs of rudder side shells which have been accomplished

in accordance with a SRM A340-200/300 procedure older than SRM April

2010 revision, must be inspected in accordance with this Service Bulletin.

NOTE: In the case of a rudder originally fitted on one aircraft (refer to AIR delivery

document) that has been removed and installed on another aircraft, it is the

responsibility of the operator to apply the required instructions contained in

this Service Bulletin to the new aircraft.

NOTE: In case of doubt, contact AIRBUS.

(1) Models

340-541 340-542 340-642

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 1

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

(2) Effectivity by MSN

0371 0376 0383 0391 0394 0410 0416-0417 0426 0431 0436 0440 0445 0449 0453

0457 0460 0464 0468 0471 0475 0478 0482 0485 0488 0492 0495 0499 0514 0517

0520 0523 0531 0534 0537 0540 0543 0547 0557 0560 0563 0566 0569 0572 0575

0577 0580 0583 0586 0601 0604 0606 0608 0611 0615 0617 0619 0622 0624 0626

0628 0630 0639 0672 0677 0681 0685 0689 0694 0698 0702 0706 0710 0715 0719

0723 0727 0736 0740 0744 0748 0753 0757 0761-0768 0771 0775 0779 0783 0787

0790 0794 0798 0804 0812 0829 0837 0846 0848 0870 0897 0902 0910 0912 0917

0924 0929 0933 0953 0960 0972 0981 0987 0993 1005 1017 1030 1040 1079 1091

1122

(3) Effectivity by Operator

The Operator/MSN relationship is provided for information only and is correct at the time

of issue in accordance with the information available to AIRBUS. Any future changes

resulting from transfer of an aircraft from one operator to another will not be reflected in

this list unless the Service Bulletin is revised for another reason.

OPERATOR MSN

06U 1091

25R 0924

36V 0391 0416

70U 0902

72W 0917

AHY 0779

AIB 0478 0492 0499 0560

CES 0468 0488 0514 0577 0586

CHH 0436 0453 0475

DLH 0482 0517 0523 0537 0540 0543 0566 0569 0580 0583 0762 0763

0767 0771 0790 0794 0812 0846 0848 0897 0972 0981 0987 1005

ETD 0748 0757 0761 0783 0829 0837 0870 0929 0933 1030 1040

HFM 0383

HFY 0910 0912

IBE 0431 0440 0460 0601 0604 0606 0617 0619 0672 0702 0727 0744

0960 0993 1017 1079 1122

QAF 0495

QTR 0715 0740 0766 0798

SAA 0410 0417 0426 0531 0534 0547 0557 0626 0630

SIA 0563

TAM 0445 0464

THA 0624 0628 0677 0681 0689 0698 0710 0719 0775 0953

UAE 0394 0457 0471 0485 0520 0572 0608 0611 0685 0694

VIR 0371 0376 0449 0575 0615 0622 0639 0706 0723 0736 0753 0764

0765 0768 0787 0804

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 2

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

(4) Configuration by MSN

MSN CONFIGURATION

0371 0376 0383 0391 0394 0410 0416 0417 0426 0431 0436

0440 0445 0449 0453 0457 0460 0464 0468 0471 0475 0478

0482 0485 0488 0492 0495 0499 0514 0517 0520 0523 0531

0534 0537 0540 0543 0547 0557 0560 0563 0566 0569 0572

0575 0577 0580 0583 0586 0601 0604 0606 0608 0611 0615

0617 0619 0622 0624 0626 0628 0630 0639 0672 0677 0681

0685 0689 0694 0698 0702 0706 0710 0715 0719 0723 0727

0736 0740 0744 0748 0753 0757 0761 0762 0763 0764 0765

0766 0767 0768 0771 0775 0779 0783 0787 0790 0794 0798

0804 0812 0829 0837 0846 0848 0870 0897 0902 0910 0912

0917 0924 0929 0933 0953 0960 0972 0981 0987 0993 1005

1017 1030 1040 1079 1091 1122

001

(5) Configuration definition

**CONF 001

Config. 001 is valid for all the aircraft given in the effectivity of this Service Bulletin as a

standard configuration.

(6) Material Effectivity

MATERIAL QTY PER A/C SEE NOTES

Consumable CMLD01 1

B. CONCURRENT REQUIREMENTS

None

C. REASON

(1) History

On AIRBUS Single Aisle, Long Range and Wide Body family aircraft, the rudder side

shell is a sandwich structure made of Carbon Fiber Reinforced Plastic (CFRP) and

Glass Fiber Reinforced Plastic (GFRP) with a honeycomb core. A case of skin damage

was reported on a composite side panel of a rudder installed on an A310 aircraft.

Investigations have shown that the damage started from a skin panel area previously

repaired in-service. This repair was performed as per A310 SRM 55-41-12 Fig. 204

procedure. The new damage has been identified as a damage between the core and the

skin in the repaired area. This new damage has developed during normal operations due

to the variation of pressure during ground-air-ground cycles.

Following the above mentioned damage scenario, it has been identified that SRM

procedures need to be improved to ensure an adequate repair quality. An improper

bonding between skin and core during a repair may lead to a damage initiation and

propagation, which may not be detectable visually. A large rudder damage, resulting

from an undetected damage growth, could affect the handling quality of the aircraft.

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 3

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

(2) Objective/Action

This Service Bulletin details the inspection procedure to inspect affected rudders fitted

on A340 aircraft for potential damage.

Different inspection procedures are necessary:

- Pulse thermography inspection

- Elasticity Laminate Checker (ELCH) inspection

- Ultrasonic Testing (UT) inspection.

- Tap test inspection.

(3) Advantages

The accomplishment of this Service Bulletin will contribute to detect potential damage

around in-service repairs accomplished on rudders made of Carbon Fiber Reinforced

Plastic (CFRP) and Glass Fiber Reinforced Plastic (GFRP) with a honeycomb core.

(4) Operational/Maintenance Consequences

None

D. DESCRIPTION

NOTE: The listed subtasks are not in sequence with the work steps.

To accomplish this Service Bulletin it is necessary to :

Task 555007-832-848-001: Inspection

(1) Check the rudder repair records

(2) Identify the type, location and size of in-service repairs on the rudder side shell

CFRP areas in case of complete repair records since rudder Entry Into Service (EIS) are

available

(3) Do a pulse thermography inspection on the complete rudder side shell CFRP areas

to identify possible rudder in-service repairs in case of repair records are not complete or

not available

(4) Do the corrective actions in case of fluid ingress detected

(5) Do the ELCH and/or UT inspection around identified repairs/fluid ingress

(6) Do terminating actions in case of no damage detected

(7) Inspect the rudder side shell upper GFRP areas

(8) Close the holes in case of drilling thru the outer skin during paint thickness

measurement

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 4

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

(9) Identify the repair size by local sanding

E. COMPLIANCE

(1) Classification

MANDATORY: Service Bulletin must be accomplished.

(2) Accomplishment Timescale

This Service Bulletin has been classified Mandatory by the issue of an Airworthiness

Directive (AD) published by the European Aviation Safety Agency (EASA). The AD must

be used as the reference document for the mandated accomplishment timescale.

Table 1, Config. 001 - Rudder special detailed inspection for repair detection

Condition Action Compliance time Repetitive interval

All aircraft Identify the Serial

Number of the installed

rudder in accordance

with the accomplishment

instructions Subtask

555007-832-201-001

Within 4 months from

original Service Bulletin

issue date

None

All aircraft Check the completeness

of the rudder repair

records

Within 4 months from

original Service Bulletin

issue date

None

All aircraft Report information

about the repair records

to AIRBUS

Within 4 months from

original Service Bulletin

issue date

None

Repair records are not

complete or not

available

Continue with the

actions given in table 2A

for CFRP areas

Refer to table 2A Refer to table 2A

Repair records are not

complete or not

available

Continue with the

actions given in table 2B

for GFRP areas

Refer to table 2B Refer to table 2B

Complete repair records

since rudder Entry Into

Service (EIS) are

available

Continue with the

actions given in table

2C for CFRP areas

Refer to table 2C Refer to table 2C

Complete repair records

since rudder EIS are

available

Continue with the

actions given in table

2D for GFRP areas

Refer to table 2D Refer to table 2D

Table 2A, Config. 001 - Repair records are not complete or not available (CFRP areas)

Condition Action Compliance time Repetitive interval

Repair records are not

complete or not

available

Report undocumented

rudder Serial Number

list to AIRBUS to get

related rudder

manufacturing rework

data

3 months in advance

before pulse

thermography inspection

is scheduled

None

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 5

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

Table 2A, Config. 001 - Repair records are not complete or not available (CFRP areas)

Condition Action Compliance time Repetitive interval

Repair records are not

complete or not

available

Make sure that the paint

thickness in all areas to

be inspected does not

exceed the limits given

in the accomplishment

instructions Subtask

555007-832-203-001

Within 24 months from

original Service Bulletin

issue date, before the

pulse thermography

inspection

None

Repair records are not

complete or not

available

Do a pulse

thermography inspection

on the complete side

shells (LH/RH) to

identify repairs in

accordance with the

accomplishment

instructions Subtask

555007-832-203-001

Within 24 months from

original Service Bulletin

issue date

None

No repair detected Report to AIRBUS

No further action

necessary in

accordance with this

Service Bulletin

Within 1 month from the

pulse thermography

inspection

None

Repairs in the booster

area =< 55000 mm2

(85.25 sq.in.) detected

Report to AIRBUS Within 1 month from the

pulse thermography

inspection

None

Repairs in the booster

area > 55000 mm2

(85.25 sq.in.) or not in

the booster area

detected during pulse

thermography inspection

Do an ELCH and/or UT

inspection around the

identified repairs in

accordance with the

accomplishment

instructions Subtask

555007-832-205-001

Within 24 months from

original Service Bulletin

issue date

None

Fluid ingress detected

during pulse

thermography/UT

inspection

Continue with the

actions given in table 3

Refer to table 3 Refer to table 3

Damage detected during

ELCH and/or UT

inspection

Provide a detailed

damage report and

report to AIRBUS and

follow their instructions

Before next flight None

No damage detected

during ELCH and/or UT

inspection

Continue with the

actions given in table 4

Refer to table 4 Refer to table 4

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 6

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

Table 2B, Config. 001 - Repair records are not complete or not available (GFRP areas)

Condition Action Compliance time Repetitive interval

Repair records are not

complete or not

available

Make sure that the paint

thickness in all areas to

be inspected does not

exceed the limits given

in the accomplishment

instructions

555007-832-207-001

Within 24 months from

original Service Bulletin

issue date, before the

pulse thermography

inspection

None

Repair records are not

complete or not

available

Do a pulse

thermography inspection

on the complete GFRP

area in accordance with

the accomplishment

instructions Subtask

555007-832-207-001

Within 24 months from

original Service Bulletin

issue date

None

Repair records are not

complete or not

available

In case of findings, mark

the repairs which are

not manufacturing

reworks

Within 24 months from

original Service Bulletin

issue date

None

Repair records are not

complete or not

available

Do a Tap test inspection

on the complete GFRP

area to identify skin to

core disbonding in

accordance with the

accomplishment

instructions Subtask

555007-832-207-001

Within 24 months from

original Service Bulletin

issue date

None

No skin to core

disbonding but repairs

identified

Do an ELCH and/or UT

inspection on the

complete GFRP area in

accordance with the

accomplishment

instructions Subtask

555007-832-205-001

Within 24 months from

original Service Bulletin

issue date

None

Fluid ingress detected

during pulse

thermography/UT

inspection

Continue with the

actions given in table 3

Refer to table 3 Refer to table 3

Damage detected during

tap test/ELCH and/or

UT inspection

Provide a detailed

damage report and

report to AIRBUS and

follow their instructions

Before next flight None

No damage detected

during tap test/ELCH

and/or UT inspection

Continue with the

actions given in table 4

Refer to table 4 Refer to table 4

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 7

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

Table 2C, Config. 001 - Repair records since rudder EIS are complete (CFRP areas)

Condition Action Compliance time Repetitive interval

No repair performed or

repair not to be

inspected in accordance

with this Service Bulletin

Report to AIRBUS

No further action

necessary in

accordance with this

Service Bulletin

Within 24 months from

original Service Bulletin

issue date

None

Repair is performed

since rudder EIS

Identify the repair type

in accordance with the

accomplishment

instructions Subtask

555007-832-202-001

Within 24 months from

original Service Bulletin

issue date

None

Repair identified as type

to be inspected

Make sure that the paint

thickness in all areas to

be inspected does not

exceed the limits given

in the accomplishment

instructions Subtask

555007-832-202-001

Within 24 months from

original Service Bulletin

issue date, before the

pulse thermography

inspection

None

Repair identified as type

to be inspected

Do a pulse

thermography inspection

on repair location in

accordance with the

accomplishment

instructions Subtask

555007-832-202-001

or

Identify the repair size

by local sanding, refer

to Subtask

555007-832-208-001

Within 24 months from

original Service Bulletin

issue date

None

Repairs in the booster

area =< 55000 mm2

(85.25 sq.in.) detected

during pulse

thermography inspection

or local sanding

Report to AIRBUS Within 1 month from

pulse thermography

inspection

None

Repairs in the booster

area > 55000 mm2

(85.25 sq.in.) or not in

the booster area

detected during pulse

thermography inspection

or local sanding

Do an ELCH and/or UT

inspection around the

identified repairs in

accordance with the

accomplishment

instructions Subtask

555007-832-205-001

Within 24 months from

original Service Bulletin

issue date

None

Fluid ingress detected

during pulse

thermography/UT

inspection

Continue with the

actions given in table 3

Refer to table 3 Refer to table 3

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 8

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

Table 2C, Config. 001 - Repair records since rudder EIS are complete (CFRP areas)

Condition Action Compliance time Repetitive interval

Damage detected during

ELCH and/or UT

inspection

Provide a detailed

damage report, report to

AIRBUS and follow their

instructions

Before next flight None

No damage detected

during ELCH and/or UT

inspection

Continue with the

actions given in table 4

Refer to table 4 Refer to table 4

Table 2D, Config. 001 - Repair records since rudder EIS are complete (GFRP areas)

Condition Action Compliance time Repetitive interval

No repair performed or

repair not to be

inspected in accordance

with this Service Bulletin

Report to AIRBUS

No further action

necessary in

accordance with this

Service Bulletin

Within 24 months from

original Service Bulletin

issue date

None

Repair performed and

identified as type to be

inspected

Make sure that the paint

thickness in all areas to

be inspected does not

exceed the limits given

in the accomplishment

instructions Subtask

555007-832-207-001

Within 24 months from

original Service Bulletin

issue date, before the

pulse thermography

inspection

None

Repair identified as type

to be inspected

Do a pulse

thermography inspection

on repair location in

accordance with the

accomplishment

instructions Subtask

555007-832-207-001

or

Identify the repair size

by local sanding, refer

to Subtask

555007-832-208-001

Within 24 months from

original Service Bulletin

issue date

None

Repair type A-A

identified

Do a Tap test inspection

on the repair in

accordance with the

accomplishment

instructions Subtask

555007-832-207-001

Within 24 months from

original Service Bulletin

issue date

None

All other repairs Do an ELCH and/or UT

inspection around the

identified repairs in

accordance with the

accomplishment

instructions Subtask

555007-832-205-001

Within 24 months from

original Service Bulletin

issue date

None

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 9

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

Table 2D, Config. 001 - Repair records since rudder EIS are complete (GFRP areas)

Condition Action Compliance time Repetitive interval

Fluid ingress detected

during pulse

thermography/UT

inspection

Continue with the

actions given in table 3

Refer to table 3 Refer to table 3

Damage detected during

tap test/ELCH and/or

UT inspection

Provide a detailed

damage report and

report to AIRBUS and

follow their instructions

Before next flight None

No damage detected

during tap test/ELCH

and/or UT inspection

Continue with the

actions given in table 4

Refer to table 4 Refer to table 4

Table 3, Config. 001 - Fluid ingress detected

Condition Action Compliance time Repetitive interval

Fluid ingress detected Do an ELCH and/or UT

inspection around the

identified fluid ingress in

accordance with the

accomplishment

instructions Subtask

555007-832-205-001

Before next flight None

Damage detected

around the identified

fluid ingress

Report to AIRBUS and

follow their instructions

Before next flight None

Local single spot fluid

ingress =< 1500 mm2

(2.33 sq.in.) detected (no

damage detected around

the identified fluid

ingress)

Report to AIRBUS Within 1 month from

pulse thermography

inspection

None

Maximum of 5 local

single spots fluid ingress

per side shell > 1500

mm2 (2.33 sq.in.) and =<

5000 mm2 (7.75 sq.in.)

detected (no damage

detected around the

identified fluid ingress)

Drain by core ventilation

in accordance with the

accomplishment

instructions Subtask

555007-832-204-001

Before next flight None

Core ventilation done Option 1:

Close the holes with

adhesive tape

Before next flight None

Holes closed with tape Option 1:

Do repetitive detailed

inspections of the

restored area for loose

or lost tape

Within 900 FH after

closing the holes

At intervals not

exceeding 900 FH

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 10

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

Table 3, Config. 001 - Fluid ingress detected

Condition Action Compliance time Repetitive interval

Loose or lost tape found Option 1:

Close the holes again

with adhesive tape or

refer to Option 2

Before next flight None

Core ventilation done Option 2:

Close the holes with

GFRP plies

Before next flight None

Maximum of 5 local

single spots fluid ingress

per side shell > 1500

mm2 (2.33 sq.in.) and =<

5000 mm2 (7.75 sq.in.)

detected (no damage

detected around the

identified fluid ingress)

Option 1 and 2:

Repetitive thermography

inspections in

accordance with the

accomplishment

instructions Subtask

555007-832-204-001

Within 1000 FC after

closing the holes

Within intervals of 1000

FC until repair

Maximum of 5 local

single spots fluid ingress

per side shell > 1500

mm2 (2.33 sq.in.) and =<

5000 mm2 (7.75 sq.in.)

detected (no damage

detected around the

identified fluid ingress)

Do the repair Within 4500 FC, but not

exceeding 24 months

from the first inspection

None

Maximum of 5 local

single spots fluid ingress

per side shell > 1500

mm2 (2.33 sq.in.) and =<

5000 mm2 (7.75 sq.in.)

detected (no damage

detected around the

identified fluid ingress)

Report to AIRBUS Within 1 month from the

repair

None

More than 5 local single

spots fluid ingress per

side shell > 1500 mm2

(2.33 sq.in.) and =<

5000 mm2 (7.75 sq.in.)

detected (no damage

detected around the

identified fluid ingress)

Report to AIRBUS and

follow their instructions

Before next flight None

Local single spot fluid

ingress > 5000 mm2

(7.75 sq.in.) detected (no

damage detected around

the identified fluid

ingress)

Report to AIRBUS and

follow their instructions

Before next flight None

Tables 4.A thru 4.D, Config. 001: No damage detected during ELCH/UT inspection:

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 11

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

For an identified repair size of a maximum of 10000 mm2 (15.50 sq.in.), continue with

table 4.A.

For an identified repair size larger than 10000 mm2 (15.50 sq.in.) and up to 20000 mm2

(31.00 sq.in.), continue with table 4.B.

For an identified repair size larger than 20000 mm2 (31.00 sq.in.) and up to 80000 mm2

(124 sq.in.), continue with table 4.C.

For an identified repair size larger than 80000 mm2 (124 sq.in.), continue with table 4.D.

Table 4.A, Config. 001 - Identified repair size of a maximum of 10000 mm2 (15.50 sq.in.)

Condition Action Compliance time Repetitive interval

Repair size =< 10000

mm2 (15.50 sq.in.)

Provide detailed

information about the

identified repair and

report to AIRBUS

Within 1 month from

ELCH/UT inspection

None

Table 4.B, Config. 001 - Identified repair size larger than 10000 mm2 (15.50 sq.in.) and up to 20000

mm2(31.00 sq.in.)

Condition Action Compliance time Repetitive interval

Repair size > 10000

mm2 (15.50 sq.in.) and

=< 20000 mm2 (31.00

sq.in.)

Option 1:

Do the core ventilation

thru the inner skin in

accordance with the

accomplishment

instructions Subtask

555007-832-206-001

Before next flight None

Core ventilation done Option 1:

Hole closing option 1:

Close the holes with

adhesive tape

Before next flight None

Holes closed with tape Option 1:

Hole closing option 1:

Do repetitive detailed

inspections of the

restored area for loose

or lost tape

Within 900 FH after

closing the holes

At intervals not

exceeding 900 FH

Loose or lost tape found Option 1:

Hole closing option 1:

Close the holes again

with adhesive tape or

refer to hole closing

option 2

Before next flight None

Core ventilation done Option 1:

Hole closing option 2:

Close the holes with

GFRP plies

Before next flight None

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 12

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

Table 4.B, Config. 001 - Identified repair size larger than 10000 mm2 (15.50 sq.in.) and up to 20000

mm2(31.00 sq.in.)

Condition Action Compliance time Repetitive interval

Core ventilation done Option 1:

Report detailed

information about the

identified repair and the

planned terminating

action to AIRBUS

Within 1 month from first

ELCH/UT inspection

None

Core ventilation done Option 1:

Do the repair in

accordance with the

SRM at the identified

repair location

Within 4500 FC, not

exceeding 24 months,

from the first inspection

date

None

Repair size > 10000

mm2 (15.50 sq.in.) and

=< 20000 mm2 (31.00

sq.in.)

Option 2:

Do repetitive ELCH/UT

inspections around the

identified repair area in

accordance with the

accomplishment

instructions Subtask

555007-832-205-001

Within 900 FH from first

ELCH/UT inspection

Every 900 FH from last

ELCH/UT inspection

Findings during

repetitive ELCH/UT

inspections

Option 2:

Report to AIRBUS and

follow their instructions

Before next flight None

No findings during

repetitive ELCH/UT

inspections

Option 2:

Report detailed

information about the

identified repair and the

planned terminating

action to AIRBUS

Within 1 month from

ELCH/UT inspection

None

No findings during

repetitive ELCH/UT

inspections

Option 2:

Do the repair in

accordance with the

SRM at the identified

repair location

Within 4500 FC, not

exceeding 24 months,

from the first inspection

date

None

Table 4.C, Config. 001 - Identified repair size larger than 20000 mm2 (31.00 sq.in.) and up to 80000

mm2 (124 sq.in.)

Condition Action Compliance time Repetitive interval

Repair size > 20000

mm2 (31.00 sq.in.) and

=< 80000 mm2 (124

sq.in.)

Do the core ventilation

thru inner skin in

accordance with the

accomplishment

instructions Subtask

555007-832-206-001

Before next flight None

Core ventilation done Option 1:

Close the holes with

adhesive tape

Before next flight None

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 13

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

Table 4.C, Config. 001 - Identified repair size larger than 20000 mm2 (31.00 sq.in.) and up to 80000

mm2 (124 sq.in.)

Condition Action Compliance time Repetitive interval

Holes closed with tape Option 1:

Do repetitive detailed

inspections of the

restored area for loose

or lost tape

Within 900 FH after

closing the holes

At intervals not

exceeding 900 FH

Loose or lost tape found Option 1:

Close the holes again

with adhesive tape or

refer to Option 2

Before next flight None

Core ventilation done Option 2:

Close the holes with

GFRP plies

Before next flight None

Repair size > 20000

mm2 (31.00 sq.in.) and

=< 80000 mm2 (124

sq.in.)

Report detailed

information about the

identified repair and the

planned terminating

action to AIRBUS

Within 1 month from first

ELCH/UT inspection

None

Core ventilation done

and repair size =<

30000 mm2 (46.50

sq.in.)

Do the repair in

accordance with the

SRM at the identified

repair location

Within 4500 FC, not

exceeding 24 months,

from the first inspection

date

None

Core ventilation done

and repair size > 30000

mm2 (46.50 sq.in.) and

=< 80000 mm2 (124

sq.in.)

Do the repair in

accordance with the

SRM and additional

instructions from

AIRBUS

Within 4500 FC, not

exceeding 24 months,

from the first inspection

date

None

Table 4.D, Config. 001 - Identified repair size larger than 80000 mm2 (124 sq.in.)

Condition Action Compliance time Repetitive interval

Repair size > 80000

mm2 (124 sq.in.)

Do the core ventilation

thru inner skin in

accordance with the

accomplishment

instructions Subtask

555007-832-206-001

Before next flight None

Core ventilation done Option 1:

Close the holes with

adhesive tape

Before next flight None

Holes closed with tape Option 1:

Do repetitive detailed

inspections of the

restored area for loose

or lost tape

Within 900 FH after

closing the holes

At intervals not

exceeding 900 FH

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 14

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

Table 4.D, Config. 001 - Identified repair size larger than 80000 mm2 (124 sq.in.)

Condition Action Compliance time Repetitive interval

Loose or lost tape found Option 1:

Close the holes again

with adhesive tape or

refer to Option 2

Before next flight None

Core ventilation done Option 2:

Close the holes with

GFRP plies

Before next flight None

Repair size > 80000

mm2 (124 sq.in.)

Report detailed

information about the

identified repair and the

planned terminating

action to AIRBUS

Within 1 month from first

ELCH/UT inspection

None

Repair size > 80000

mm2 (124 sq.in.)

Replace the affected

rudder shell

OR

Replace the rudder

No further action

necessary in

accordance with this

Service Bulletin

Within 4500 FC, not

exceeding 24 months,

from the first inspection

date

None

Table 5, Config. 001 - Hole closing in case of damaged outer skin during paint thickness

measurement

Condition Action Compliance time Repetitive interval

Sandwich structure

damaged

Option 1:

Close the holes with

resin and adhesive tape

Before next flight None

Holes closed Option 1:

Restore the surface

protection

Within 4500 FC from the

pulse thermography

inspection

None

Sandwich structure

damaged

Option 2:

Do the permanent

restoration procedure

Before next flight None

Table 6.A, Config. 001 - Identify the repair size by local sanding

Condition Action Compliance time Repetitive interval

Repair performed and

identified as type to be

inspected

Identify paint thickness

and primer

Within 24 months from

original Service Bulletin

issue date

None

Repair performed and

identified as type to be

inspected

Do local sanding on top

and around the repair

up to the initial basic

primer

Within 24 months from

original Service Bulletin

issue date

None

Largest repair ply is not

visible

Continue with the

actions given in table

6.B

Before next flight None

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 15

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

Table 6.A, Config. 001 - Identify the repair size by local sanding

Condition Action Compliance time Repetitive interval

Largest repair ply is

visible

Remove the dust and

dry the area

Before next flight None

Largest repair ply is

visible

Inspect the sanded area

for damage

Before next flight None

Damage found Do the damage

assessment

Before next flight None

No damage found Mark the repair on the

rudder surface

Before next flight None

Repairs in the booster

area =< 55000 mm2

(85.25 sq.in.) detected

Restore the surface

protection

Before next flight None

Repairs in the booster

area =< 55000 mm2

(85.25 sq.in.) detected

Report to AIRBUS Within 1 month None

Repairs in the booster

area > 55000 mm2

(85.25 sq.in.) or not in

the booster area

detected

Do an ELCH and/or UT

inspection around the

identified repairs in

accordance with the

accomplishment

instructions Subtask

555007-832-205-001

Before next flight None

Fluid ingress detected

during UT inspection

Continue with the

actions given in table 3

Refer to table 3 Refer to table 3

Damage detected during

ELCH and/or UT

inspection

Provide a detailed

damage report, report to

AIRBUS and follow their

instructions

Before next flight None

No damage detected

during ELCH and/or UT

inspection

Continue with the

actions given in table 4

Refer to table 4 Refer to table 4

Table 6.B, Config. 001 - Identify the repair size by local sanding - largest repair ply not visible

Condition Action Compliance time Repetitive interval

Largest repair ply is not

visible

Continue local sanding

up to the pore

filler/adhesive

Before next flight None

Largest repair ply is

visible now

Remove the dust and

dry the area

Before next flight None

Largest repair ply is still

not visible

Continue with the

actions given in table

6.C for CFRP areas and

table 6.D for GFRP

areas

Before next flight None

Largest repair ply is

visible now

Inspect the sanded area

for damage

Before next flight None

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 16

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

Table 6.B, Config. 001 - Identify the repair size by local sanding - largest repair ply not visible

Condition Action Compliance time Repetitive interval

Damage found Do the damage

assessment

Before next flight None

No damage found Mark the repair on the

rudder surface

Before next flight None

Repairs in the booster

area =< 55000 mm2

(85.25 sq.in.) detected

Restore the surface

protection

Before next flight None

Repairs in the booster

area =< 55000 mm2

(85.25 sq.in.) detected

Report to AIRBUS Within 1 month None

Repairs in the booster

area > 55000 mm2

(85.25 sq.in.) or not in

the booster area

detected

Do an ELCH and/or UT

inspection around the

identified repairs in

accordance with the

accomplishment

instructions Subtask

555007-832-205-001

Before next flight None

Fluid ingress detected

during UT inspection

Continue with the

actions given in table 3

Refer to table 3 Refer to table 3

Damage detected during

ELCH and/or UT

inspection

Provide a detailed

damage report, report to

AIRBUS and follow their

instructions

Before next flight None

No damage detected

during ELCH and/or UT

inspection

Continue with the

actions given in table 4

Refer to table 4 Refer to table 4

Table 6.C, Config. 001 - Do the pulse thermography inspection (CFRP areas)

Condition Action Compliance time Repetitive interval

Largest repair ply is still

not visible

Do a pulse

thermography inspection

on repair location in

accordance with the

accomplishment

instructions Subtask

555007-832-202-001

Before next flight None

Repairs in the booster

area =< 55000 mm2

(85.25 sq.in.) detected

during pulse

thermography inspection

Restore the surface

protection

Before next flight None

Repairs in the booster

area =< 55000 mm2

(85.25 sq.in.) detected

during pulse

thermography inspection

Report to AIRBUS Within 1 month None

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 17

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

Table 6.C, Config. 001 - Do the pulse thermography inspection (CFRP areas)

Condition Action Compliance time Repetitive interval

Repairs in the booster

area > 55000 mm2

(85.25 sq.in.) or not in

the booster area

detected during pulse

thermography inspection

Do an ELCH and/or UT

inspection around the

identified repairs in

accordance with the

accomplishment

instructions Subtask

555007-832-205-001

Before next flight None

Fluid ingress detected

during pulse

thermography/UT

inspection

Continue with the

actions given in table 3

Refer to table 3 Refer to table 3

Damage detected during

ELCH and/or UT

inspection

Provide a detailed

damage report, report to

AIRBUS and follow their

instructions

Before next flight None

No damage detected

during ELCH and/or UT

inspection

Continue with the

actions given in table 4

Refer to table 4 Refer to table 4

Table 6.D, Config. 001 - Do the pulse thermography inspection (GFRP areas)

Condition Action Compliance time Repetitive interval

Repair identified as type

to be inspected

Do a pulse

thermography inspection

on repair location in

accordance with the

accomplishment

instructions Subtask

555007-832-207-001

Before next flight None

Repair type A-A

identified

Do a Tap test inspection

on the identified repair

in accordance with the

accomplishment

instructions Subtask

555007-832-207-001

Before next flight None

All other repairs Do an ELCH and/or UT

inspection around the

identified repairs in

accordance with the

accomplishment

instructions Subtask

555007-832-205-001

Before next flight None

Fluid ingress detected

during pulse

thermography/UT

inspection

Continue with the

actions given in table 3

Refer to table 3 Refer to table 3

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 18

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

Damage detected during

Tap test/ELCH and/or

UT inspection

Provide a detailed

damage report, report to

AIRBUS and follow their

instructions

Before next flight None

No damage detected

during ELCH and/or UT

inspection

Continue with the

actions given in table 4

Refer to table 4 Refer to table 4

F. APPROVAL

The technical content of this document is approved under authority of Design Organization

Approval No. EASA.21J.031.

If an aircraft listed in the effectivity has a modification or repair embodied that is not of

AIRBUS origin, and which affects the content of this Service Bulletin, the operator is

responsible for obtaining approval by its airworthiness authority for any adaptation necessary

before incorporation of the Service Bulletin.

G. MANPOWER

The manpower estimates given in this Service Bulletin are based on the direct labor cost to

do the work. These estimates assume that the work will be done by experienced personnel,

and may need to be revised upwards to suit operator’s circumstances. The estimates do not

include the time to prepare, plan or inspect the work. Manufacture and procurement of parts

and tools, drying times for paints, sealants, etc., and general administration work are also not

included.

Task 555007-832-848-001: Inspection

Get Access 1.00

On Aircraft

Check the rudder repair records 4.00

Identify the type, location and size of in-service repairs

on the rudder side shell CFRP areas in case of

complete repair records since rudder Entry Into Service

(EIS) are available

0

Do a pulse thermography inspection on the complete

rudder side shell CFRP areas to identify possible

rudder in-service repairs in case of repair records are

not complete or not available

32.00

Do the corrective actions in case of fluid ingress

detected

0

Do the ELCH and/or UT inspection around identified

repairs/fluid ingress

0

Do terminating actions in case of no damage detected 0

Inspect the rudder side shell upper GFRP areas 0

Close the holes in case of drilling thru the outer skin

during paint thickness measurement

0

Identify the repair size by local sanding 0

Close-Up 1.00

TOTAL MANHOURS 38.00

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 19

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

NOTE: Manhours and elapsed time depend on the size of the area to be inspected.

Find below a table with the information for the manhours, elapsed time

and number of persons per 1 m2 (1550 sq.in.) for the different inspection

procedures:

Steps Manhours Elapsed time Number of

persons

Get access 1.00 0.75 2

Rudder SN

identification

0.25 0.25 1

Pulse

thermography

inspection

1.00 0.50 2

UT inspection 1.25 1.25 1

ELCH inspection 1.50 0.75 1

Tap test inspection 0.25 0.25 1

Local sanding 1.00 1.00 1

Close-up 1.00 0.75 2

H. WEIGHT AND BALANCE

Not Changed

I. ELECTRICAL LOAD DATA

Not Changed

J. REFERENCES

Aircraft Maintenance Manual (AMM) 06-41-55 12-34-24 20-16-00

29-00-00 55-40-00

Consumable Material List (CML)

Elec. Std. Practices Manual (ESPM) 20-55-00

Non Destructive Test Manual (NTM) 51-10-03 51-10-19 51-10-24

51-10-25 51-10-26 55-40-09

55-40-50

Structural Repair Manual (SRM) 51-23-11 51-75-11 51-75-12

51-77-10 51-77-11

K. PUBLICATION AFFECTED

None

L. INTERCHANGEABILITY/MIXABILITY

Not Applicable

M. SPARES

None

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 20

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

2. MATERIAL INFORMATION

**CONF ALL

A. MATERIAL - PRICE AND AVAILABILITY

(1) Procurement Addresses

None

This Service Bulletin is the subject of an AIRBUS monitored retrofit campaign.

(2) Price and Availability

None

B. INDUSTRY SUPPORT INFORMATION

For the organisation of this retrofit, you are kindly requested to contact AIRBUS retrofit

management department:

AIRBUS

CUSTOMER SERVICES DIRECTORATE

1 Rond Point Maurice Bellonte

31707 BLAGNAC CEDEX

France

E-mail : monitored.retrofit@airbus.com

Tel : (33) 5 67 19 06 22

Fax : (33) 5 61 93 27 45

AIRBUS will provide specific industry support for inspection Service Bulletin completion. For

detailed information, please contact your AIRBUS Customer Support Director.

C. LIST OF COMPONENTS

No Kit

D. LIST OF MATERIALS - OPERATOR SUPPLIED

(1) Consumable Materials

Consumable CMLD01

ITEM DESCRIPTION REFERENCE TO CML

MAT. No.

QTY PER A/C SEE

NOTES

Adhesive Film Tape- Aluminium Foil 05RAB9 As required

Pressure Sensitive Tape 05RFB1 As required

Self-Adhes. Disks 05TNB1 As required

Non Aqueous Cleaner-General 08BAA9 As required

Methyl-Ethyl-Ketone 08BBF1 As required

Trichloroethane Legacy 08BBU9 As required

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 21

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

ITEM DESCRIPTION REFERENCE TO CML

MAT. No.

QTY PER A/C SEE

NOTES

Laminating Resin-Epoxy Srm Type

2 -

13EBC1 As required

Textile-Lint Free Cotton 14SBA1 As required

(2) Components

None

(3) Equipment

None

E. PARTS TO BE RE-IDENTIFIED BY OPERATOR

None

F. TOOLING

(1) Tooling - Price and Availability

Not Applicable

(2) Tools

To find the correct tool-PN for the different inspection tools, refer to the subsequent

table:

Inspection tool PN

UT inspection UT-equipment Refer to NTM 51-10-24

Tap test inspection Tap test inspection tool Refer to NTM 51-10-03

Tap test inspection (with

Woodpecker)

Function test block

and

Woodpecker

Refer to NTM 51-10-19

ELCH inspection Elasticity Laminate Checker Kit Refer to NTM 51-10-26

Pulse thermography inspection Pulse thermography kit 99A55407324000

Thermography inspection Thermography kit Refer to NTM 51-10-25

Paint thickness measurement Paint Borer Kit Model 518 or 518S or 518MC

with drill measuring range 10 to

1000 and 20 to 2000 microns

To order the pulse thermography kit and the paint borer kit, contact:

For tools on loan:

AIRBUS Material, Logistics and Suppliers

Lease Tool Service

Weg beim Jaeger 150

D-22335 HAMBURG

Germany

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 22

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

For ordering by internet: http.//spares.airbus.com

For ordering by E-mail: tool.lease@airbus.com

For ordering by fax: +49 40 5076 3225

For tools to buy:

AIRBUS Material, Logistics and Suppliers

IFD- In Flight Desk

Weg beim Jaeger 150

D-22335 HAMBURG

Germany

For ordering by internet: http.//spares.airbus.com

For ordering by E-mail: ifd.spares@airbus.com

For ordering by fax: +49 40 5076 4012

(3) Special Tools

None

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 23

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

This Page Intentionally Left Blank

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 24

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

3. ACCOMPLISHMENT INSTRUCTIONS

Task 555007-832-848-001 - Inspection

WARNING: MAKE SURE THAT YOU OBEY ALL THE WARNINGS AND ALL THE CAUTIONS

INCLUDED IN THE REFERENCED PROCEDURES.

WARNING: OBEY THE MANUFACTURERS INSTRUCTIONS WHEN YOU USE CLEANING

AGENTS, ADHESIVES, SEALANTS AND PAINTS. THESE MATERIALS ARE

DANGEROUS.

WARNING: WEAR THE CORRECT PROTECTIVE GLOVES, GOGGLES AND FILTER MASKS

WHEN YOU USE CLEANING AGENTS, ADHESIVES, SEALANTS AND PAINTS.

THESE MATERIALS ARE DANGEROUS.

CAUTION: ALWAYS OBEY THE PRECAUTIONS THAT FOLLOW TO KEEP

ELECTRICAL WIRING IN A SATISFACTORY CONDITION (ELECTRICALLY

AND MECHANICALLY SERVICEABLE). WHEN YOU DO MAINTENANCE

WORK, REPAIRS OR MODIFICATIONS, ALWAYS KEEP ELECTRICAL WIRING,

COMPONENTS AND THE WORK AREA AS CLEAN AS POSSIBLE. TO DO

THIS:

PUT PROTECTION, SUCH AS PLASTIC SHEETING, CLOTHS, ETC; AS

NECESSARY ON WIRING AND COMPONENTS.

REGULARLY REMOVE ALL SHAVINGS, UNWANTED MATERIAL AND OTHER

CONTAMINATION.

THESE PRECAUTIONS WILL DECREASE THE RISK OF CONTAMINATION

AND DAMAGE TO THE ELECTRICAL WIRING INSTALLATION.

IN CASE OF CONTAMINATION REFER TO ESPM 20-55-00.

NOTE: The accomplishment instructions of this Service Bulletin refer to procedures

included in other AIRBUS documents. When the words ’refer to’ are used and the

operator has an accepted alternative procedure, the accepted alternative procedure

can be used. When the words ’in accordance with’ are included in the instruction,

the procedure in the AIRBUS document must be used.

NOTE: The access and close-up instructions, not comprising return to service tests, in this

Service Bulletin do not constitute or affect the technical intent of the Service

Bulletin. Operators can therefore, as deemed necessary, omit or add access and/or

close-up steps to add flexibility to their maintenance operations as long as the

technical intent of the Service Bulletin is met within the set parameters.

NOTE: Manual titles given in the accomplishment instructions are referred to by acronyms.

Refer to paragraph 1.J., References, for the definition of acronyms.

NOTE: The purpose of flow charts is to supplement the information given in the Procedure

and Compliance paragraphs and not to serve as the primary source for tasks or

compliance times given in this Service Bulletin.

NOTE: This Service Bulletin is classified mandatory or expected to be classified mandatory

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 25

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

by an Airworthiness Directive (AD). The paragraphs 3.C. and 3.D. in these

accomplishment instructions are Required for Compliance (RC) and must be done

to comply with the AD. Other paragraphs are recommended and may be deviated

from, done as part of other actions or done with accepted methods different from

those given in the Service Bulletin, as long as the RC paragraphs can be done and

the aircraft can be put back into a serviceable condition.

Task Associated Data

Manpower

TOTAL MANHOURS 38.00

A. GENERAL

(1) Subtask 555007-910-201-001 - Standard Practices

Manpower Resources

Skills NON SPECIFIC

References

Aircraft Maintenance Manual (AMM) 06-41-55, Page Block 001

Task 20-16-00-912-801

Consumable Material List (CML)

(a) For location of the access panels refer to AMM 06-41-55, Page Block 001.

(b) For the specification of consumable materials (Mat. No.) given in this Service

Bulletin refer to Consumable Material List (CML).

(c) For circuit breaker safety practices refer to AMM Task 20-16-00-912-801.

(d) The purpose of flow charts are for information only to show the vario/Repair phases

described in this Service Bulletin.

(2) Subtask 555007-839-201-001 - Administrative

Manpower Resources

Skills NON SPECIFIC

Write in the applicable aircraft records that you have done all the work given in this

Service Bulletin.

B. PREPARATION

(1) Subtask 555007-941-201-001 - Job Set-up

Manpower Resources

Skills NON SPECIFIC

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 26

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

References

Aircraft Maintenance Manual (AMM) Task 12-34-24-860-802

Task 29-00-00-864-801

Task 29-00-00-864-802

Task 29-00-00-864-803

55-40-00, Page Block 601

NOTE: The items given in this note shall be considered as the basic Aircraft

configuration before you start a maintenance task:

- Aircraft on the ground resting on landing gear (the ground safety

locks and the wheel chocks are in position on the landing gear).

- Engine shut down, thrust reversers closed and locked.

- Aircraft in clean configuration.

- Parking brake applied.

- Aircraft electrical network de-energized.

- Hydraulic systems depressurized.

- Access to the cockpit and cabin is available.

- All circuit breakers are in closed position.

- All controls in NORM, AUTO or OFF position.

(a) Make sure that the aircraft is electrically grounded, refer to AMM Task

12-34-24-860-802.

(b) In the cockpit, put warning notices in position to tell persons not to operate the flight

controls.

(c) Open, safety and tag the circuit breakers as given in the rudder inspection/check

Job Set-up procedure, refer to AMM 55-40-00, Page Block 601.

(d) Depressurize the Green Hydraulic System, refer to AMM Task 29-00-00-864-801.

(e) Depressurize the Blue Hydraulic System, refer to AMM Task 29-00-00-864-802.

(f) Depressurize the Yellow Hydraulic System, refer to AMM Task 29-00-00-864-803.

(g) Put a warning notice in the cockpit to tell persons not to pressurize the hydraulic

systems.

(h) Put access platform(s) in position at the rudder.

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 27

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

C. PROCEDURE

(1) Subtask 555007-832-201-001 - Check the rudder repair records

Manpower Resources

Manhours 4.00

Minimum number of person 1

Subtask elapsed time 4.00

Skills NON DESTRUCTIVE

TESTING

References

Fig. A-GBAAA

Rudder SN identification

Sheet 01

Fig. A-GBCAA

Repair type identification

Sheet 01 - SRM list

Fig. A-GBHAA

Report sheet and sketches

Sheet 01 - Pulse thermography report sheet

Sheet 02 - Repair records report sheet

Sheet 03

Sheet 04

Fig. A-GBJAA

GFRP area location

Sheet 01

Sheet 02

(a) Identify the Serial Number (SN) and the Part Number (PN) of the installed rudder.

1 Check the Aircraft Inspection Report and the maintenance records to verify the

rudder identification and a potential rudder swap since EIS.

2 In case of doubts, check the rudder identification plate on the aircraft, as

shown on Fig. A-GBAAA Sheet 01.

3 If you do not find a SN/PN placard on the rudder, contact AIRBUS for further

instructions.

(b) Check the completeness of the rudder records and report the result to AIRBUS.

Use the report sheet Fig. A-GBHAA Sheet 02.

NOTE: This action is not necessary, if the information has been already

sent to AIRBUS in accordance with the OIT 999.0071/10 and the

situation did not change since then.

(c) Check the rudder records if repairs are recorded since rudder EIS.

1 Repairs not affected by this Service Bulletin are those which:

- have been covered by AIRBUS Repair Design Approval Sheet (RDAS)

after April 2010,

- have been accomplished in accordance with the SRM A340 200/300 as

listed in Fig. A-GBCAA Sheet 01,

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 28

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

- have been done in accordance with the SRM A340 200/300 revision April

2010 or later.

2 Report the result to AIRBUS. Use the report sheet Fig. A-GBHAA Sheet 02.

NOTE: This action is not necessary, if the information has been

already sent to AIRBUS in accordance with the OIT

999.0071/10 and the situation did not change since then.

3 If repairs are recorded and the repair records are complete, refer to:

- Subtask 555007-832-201-001 of this Service Bulletin for the rudder side

shell areas made of CFRP.

- Subtask 555007-832-207-001 of this Service Bulletin for the upper rudder

side shell areas made of GFRP.

NOTE: The outer skin ply of the upper area of the rudders is made

of GFRP. GFRP areas require different pulse thermography

inspection parameter than CFRP areas and additionally

Tap test inspection or Woodpecker inspection have to be

performed. For the identification of the GFRP areas, refer to

Fig. A-GBJAA Sheet 02.

4 If no repairs have been duly recorded, report the result to AIRBUS. Use the

report sheet Fig. A-GBHAA Sheet 02.

No further action is necessary in accordance with this Service Bulletin.

5 In case of any doubts about the accomplishment of repairs, refer to:

- Subtask 555007-832-203-001 of this Service Bulletin for the rudder side

shell areas made of CFRP.

- Subtask 555007-832-207-001 of this Service Bulletin for the upper rudder

side shell areas made of GFRP.

6 If the repair records are not complete or not available, refer to:

- Subtask 555007-832-203-001 of this Service Bulletin for the rudder side

shell areas made of CFRP.

- Subtask 555007-832-207-001 of this Service Bulletin for the upper rudder

side shell areas made of GFRP.

NOTE: The outer skin ply of the upper area of the rudders is made

of GFRP. GFRP areas require different pulse thermography

inspection parameter than CFRP areas and additionally

Tap test inspection or Woodpecker inspection have to be

performed. For the identification of the GFRP areas, refer to

Fig. A-GBJAA Sheet 02.

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 29

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

(2) Subtask 555007-832-202-001 - Identify the type, location and size of in-service

repairs on the rudder side shell CFRP areas in case of complete repair records

since rudder Entry Into Service (EIS) are available

Manpower Resources

Manhours 0

Minimum number of person 2

Subtask elapsed time 0

Skills NON DESTRUCTIVE

TESTING

Material necessary to do the job

Consumable CMLD01

ITEM DESCRIPTION REFERENCE TO

CML MAT. No.

QTY PER A/C SEE

NOTES

Non Aqueous CleanerGeneral08BAA9 As required

Textile-Lint Free Cotton 14SBA1 As required

References

Non Destructive Test Manual (NTM) Task 55-40-50-290-801

Structural Repair Manual (SRM) 51-75-11

51-75-12

Fig. A-GBBAA

Repair type identification

Sheet 01

Sheet 02

Fig. A-GBDAA

Booster area definition

Sheet 01

Sheet 02

Sheet 03

Fig. A-GBEAA

Typical pulse thermography and

ELCH/UT inspection

Sheet 01

Sheet 02 - Repair size assessment

Sheet 03 - Repair size assessment

Sheet 04 - Boundary and grid of ELCH/UT

inspections

Sheet 05 - ELCH inspection grid

Fig. A-GBHAA

Report sheet and sketches

Sheet 01 - Pulse thermography report sheet

Sheet 02 - Repair records report sheet

Sheet 03

Sheet 04

Fig. A-GFAAA

Flow Chart

Sheet 01 - Flow Chart 1

Sheet 02 - Flow Chart 2

Sheet 03 - Flow Chart 3

Sheet 04 - Flow Chart 4

Sheet 05 - Flow Chart 5

Sheet 06

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 30

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

References

Fig. A-GABAA

Paint borer instructions

Sheet 01

Sheet 02

Sheet 03

Sheet 04

Sheet 05

Sheet 06

Sheet 07

Sheet 08

(a) If no repair has been done or the recorded repair is not to be inspected in

accordance with this Service Bulletin, report to AIRBUS. Use the report sheet Fig.

A-GBHAA Sheet 02.

NOTE: This action is not necessary, if the information has been already

sent to AIRBUS in accordance with the OIT 999.0071/10 and the

situation did not change since then.

No further action is necessary in accordance with this Service Bulletin.

(b) If a repair must be inspected in accordance with this Service Bulletin, do the

subsequent work steps in accordance with the Flow Chart Fig. A-GFAAA Sheet 01:

1 Identify the repair type, refer to Fig. A-GBBAA Sheet 01 and Fig. A-GBBAA

Sheet 02.

2 Make sure that the paint thickness in the areas to be inspected by pulse

thermography does not exceed:

- 800 microns.

- 400 microns below the decal foil if a decal foil is installed.

NOTE: It is the responsibility of the operator to ensure that the paint

thickness in all areas to be inspected is below or equal to the

limits given above.

a If the paint coating and/or logo application is too thick, abrade the paint in

accordance with the SRM 51-75-11 to a thickness below or equal to the

limits given above.

NOTE: Chemical paint stripping is not allowed.

b In case of doubts about the paint thickness, measure the thickness using

a Paint Borer Kit, refer to the Figure Fig. A-GABAA Sheet 01 thru Fig. AGABAA Sheet 08.

<1>

CAUTION: DO NOT DRILL DEEPLY INTO THE BASE

MATERIAL (CFRP OR GFRP). DRILLING TOO

DEEP LEADS TO DAMAGE IN THE OUTER SKIN

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 31

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

If you damage the outer skin with the paint borer, refer to the

Subtask 555007-833-201-001 for repair instructions.

3 Clean the areas to be inspected with:

Non Aqueous

Cleaner-General

08BAA9 As required

and

Textile-Lint Free

Cotton

14SBA1 As required

4 Do a pulse thermography inspection to get the precise location and the size of

the repair, refer to NTM Task 55-40-50-290-801.

NOTE: As an alternative for the pulse thermography inspection, you

can identify the repair size by local sanding, refer to Subtask

555007-832-208-001.

NOTE: The pulse thermography inspection indicates the outer skin

repair ply geometry. The largest repair ply defines the

boundary of the repair area.

NOTE: In case of any findings (repair, damage, fluid ingress) during

the pulse thermography inspection, save the images and send

it together with the report sheet to AIRBUS.

5 Mark the boundary of the repair area, refer to Fig. A-GBEAA Sheet 02 and

Fig. A-GBEAA Sheet 03.

6 If fluid ingress has been detected during the pulse thermography inspection,

refer to Subtask 555007-832-204-001 of this Service Bulletin.

7 Identify the booster areas in accordance with Fig. A-GBDAA Sheet 02 and Fig.

A-GBDAA Sheet 03.

8 If repairs in the booster areas up to 55000 mm2 (85.25 sq.in.) have been

detected, report the findings to AIRBUS. Use the report sheet Fig. A-GBHAA

Sheet 01 and the rudder related sketches, refer to Fig. A-GBHAA Sheet 03

and Fig. A-GBHAA Sheet 04.

No further actions on these repairs in accordance with this Service Bulletin.

9 If repairs in the booster areas larger than 55000 mm2 (85.25 sq.in.) have been

detected, do the UT inspection around the repair in accordance with Subtask

555007-832-205-001 of this Service Bulletin.

10 If repairs not in the booster area have been detected, do the ELCH and/or UT

inspection in accordance with Subtask 555007-832-205-001 of this Service

Bulletin.

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 32

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

11 After the inspection, restore the paint coating in accordance with the SRM

51-75-12.

NOTE: Refer to OIT 999.0130/06 ’paint system - best practices’.

(3) Subtask 555007-832-203-001 - Do a pulse thermography inspection on the

complete rudder side shell CFRP areas to identify possible rudder in-service

repairs in case of repair records are not complete or not available

Manpower Resources

Manhours 32.00

Minimum number of person 2

Subtask elapsed time 16

Skills NON DESTRUCTIVE

TESTING

Material necessary to do the job

Consumable CMLD01

ITEM DESCRIPTION REFERENCE TO

CML MAT. No.

QTY PER A/C SEE

NOTES

Non Aqueous CleanerGeneral08BAA9 As required

Textile-Lint Free Cotton 14SBA1 As required

References

Non Destructive Test Manual (NTM) Task 55-40-50-290-801

Structural Repair Manual (SRM) 51-75-11

51-75-12

Fig. A-GFAAA

Flow Chart

Sheet 01 - Flow Chart 1

Sheet 02 - Flow Chart 2

Sheet 03 - Flow Chart 3

Sheet 04 - Flow Chart 4

Sheet 05 - Flow Chart 5

Sheet 06

Fig. A-GBDAA

Booster area definition

Sheet 01

Sheet 02

Sheet 03

Fig. A-GBHAA

Report sheet and sketches

Sheet 01 - Pulse thermography report sheet

Sheet 02 - Repair records report sheet

Sheet 03

Sheet 04

Fig. A-GABAA

Paint borer instructions

Sheet 01

Sheet 02

Sheet 03

Sheet 04

Sheet 05

Sheet 06

Sheet 07

Sheet 08

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 33

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

(a) Do the subsequent work steps in accordance with the Flow Chart Fig. A-GFAAA

Sheet 01:

1 Report undocumented rudder S/N list to AIRBUS.

a To get related rudder manufacturing rework data, provide AIRBUS

with the rudder P/N, S/N and aircraft MSN in accordance with the

accomplishment timescale instructions, refer to Para 1.E table 2A of this

Service Bulletin.

The manufacturing rework data will be provided through drawings

covered by Mod. 202490.

2 Make sure that the paint thickness in the areas to be inspected by pulse

thermography does not exceed:

- 800 microns.

- 400 microns below the decal foil if a decal foil is installed.

NOTE: It is the responsibility of the operator to ensure that the paint

thickness in all areas to be inspected is below or equal to the

limits given above.

a If the paint coating and/or logo application is too thick, abrade the paint in

accordance with the SRM 51-75-11 to a thickness below or equal to the

limits given above.

NOTE: Chemical paint stripping is not allowed.

b In case of doubts about the paint thickness, measure the thickness using

a Paint Borer Kit, refer to the Figure Fig. A-GABAA Sheet 01 thru Fig. AGABAA Sheet 08.

<1>

CAUTION: DO NOT DRILL DEEPLY INTO THE BASE

MATERIAL (CFRP OR GFRP). DRILLING TOO

DEEP LEADS TO DAMAGE IN THE OUTER SKIN

If you damage the outer skin with the paint borer, refer to the

Subtask 555007-833-201-001 for repair instructions.

3 Clean the areas to be inspected with:

Non Aqueous

Cleaner-General

08BAA9 As required

and

Textile-Lint Free

Cotton

14SBA1 As required

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 34

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

4 Do a pulse thermography inspection on the complete side shell CFRP areas

(LH/RH) to identify repairs, refer to NTM Task 55-40-50-290-801.

NOTE: The pulse thermography inspection indicates the outer skin

repair ply geometry. The largest repair ply defines the

boundary of the repair area.

NOTE: In case of any findings (repair, damage, fluid ingress) during

the pulse thermography inspection, save the images and send

it together with the report sheet to AIRBUS.

5 If no repair has been detected during the pulse thermography inspection,

report the result to AIRBUS. Use the report sheet Fig. A-GBHAA Sheet 01.

No further action is necessary in accordance with this Service Bulletin.

6 If fluid ingress has been detected during the thermograhy inspection, refer to

Subtask 555007-832-204-001 of this Service Bulletin.

7 Identify the booster areas in accordance with Fig. A-GBDAA Sheet 02 and Fig.

A-GBDAA Sheet 03.

8 If repairs in the booster areas up to 55000 mm2 (85.25 sq.in.) have been

detected which are not manufacturing rework, report the findings to AIRBUS.

Use the report sheet Fig. A-GBHAA Sheet 01 and the rudder related sketches,

refer to Fig. A-GBHAA Sheet 03 and Fig. A-GBHAA Sheet 04.

No further actions on these repairs in accordance with this Service Bulletin.

9 If repairs in the booster areas larger than 55000 mm2 (85.25 sq.in.) have been

detected which are not manufacturing rework, do the UT inspection around the

repairs in accordance with the Subtask 555007-832-205-001 of this Service

Bulletin.

10 If repairs have been detected during the pulse thermography inspection which

are not manufacturing rework and not in the booster areas, do the ELCH

and/or UT inspection around the repairs in accordance with the Subtask

555007-832-205-001 of this Service Bulletin.

11 After the inspection, restore the paint coating in accordance with the SRM

51-75-12.

NOTE: Refer to OIT 999.0130/06 ’paint system - best practices’.

(4) Subtask 555007-832-204-001 - Do the corrective actions in case of fluid ingress

detected

Manpower Resources

Manhours 0

Minimum number of person 1

Subtask elapsed time 0

Skills NON DESTRUCTIVE

TESTING

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 35

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

Material necessary to do the job

Consumable CMLD01

ITEM DESCRIPTION REFERENCE TO

CML MAT. No.

QTY PER A/C SEE

NOTES

Adhesive Film TapeAluminium Foil05RAB9 As required

Pressure Sensitive Tape 05RFB1 As required

Self-Adhes. Disks 05TNB1 As required

Methyl-Ethyl-Ketone 08BBF1 As required

Trichloroethane Legacy 08BBU9 As required

Laminating Resin-Epoxy

Srm Type 2 -

13EBC1 As required

References

Non Destructive Test Manual (NTM) 51-10-25

Task 55-40-50-290-801

Fig. A-GFAAA

Flow Chart

Sheet 01 - Flow Chart 1

Sheet 02 - Flow Chart 2

Sheet 03 - Flow Chart 3

Sheet 04 - Flow Chart 4

Sheet 05 - Flow Chart 5

Sheet 06

Fig. A-GBHAA

Report sheet and sketches

Sheet 01 - Pulse thermography report sheet

Sheet 02 - Repair records report sheet

Sheet 03

Sheet 04

Fig. A-GBFAA

Core ventilation procedure

Sheet 01

Sheet 02

Sheet 03

Fig. A-GAAAA

Closing of ventilation holes

Sheet 01

Sheet 02

(a) If fluid ingress has been detected, continue with the subsequent work steps in

accordance with the Flow Chart Fig. A-GFAAA Sheet 03:

1 Around the identified fluid ingress, do the ELCH and/or UT inspection in

accordance with the Subtask 555007-832-205-001 of this Service Bulletin.

2 If a damage has been detected during the ELCH and/or UT inspection, contact

AIRBUS and follow their instructions. Use the report sheet Fig. A-GBHAA

Sheet 01.

3 If local single spots up to 1500 mm2 (2.33 sq.in.) with fluid ingress have been

detected, report the findings to AIRBUS. Use the report sheet Fig. A-GBHAA

Sheet 01 and the rudder related sketches, refer to Fig. A-GBHAA Sheet 03

and Fig. A-GBHAA Sheet 04.

No further actions on these local single spots of fluid ingress in accordance

with this Service Bulletin.

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 36

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

4 If a maximum of 5 local single spots per side shell larger than 1500 mm2 (2.33

sq.in.) and up to 5000 mm2 (7.75 sq.in.) have been detected, do the ventilation

of the rudder core:

a

CAUTION: TO DRILL THE HOLES APPLY MODERATE

PRESSURE TO PREVENT DAMAGE TO THE SKIN, AT

THE END OF THE DRILLING OPERATION. DO NOT

DRILL THE OPPOSITE SHELL.

Drill the holes to a DIA of 3.0 mm (0.12 in.) through the outer and inner

skin in accordance with the dimensions shown on Fig. A-GBFAA Sheet

02 and Fig. A-GBFAA Sheet 03.

NOTE: Spots of fluid ingress behind the trailing edge screw line

must not be vented.

b Temporary restoration of the drain holes option 1:

<1> Close the drain holes with:

Adhesive Film

Tape- Aluminium

Foil

05RAB9 As required

or

Self-Adhes. Disks 05TNB1 As required

<2> Do repetitive detailed inspections of the restored area for loose or

lost adhesive disks or tape until the repair of the affected area has

been done.

<3> In case of loose or lost tape or disks, close the holes again with:

Adhesive Film

Tape- Aluminium

Foil

05RAB9 As required

or

Self-Adhes. Disks 05TNB1 As required

c Temporary restoration of the drain holes option 2:

<1> Close the drain holes in accordance with the instructions given in

the Figure Fig. A-GAAAA Sheet 01 and Fig. A-GAAAA Sheet 02.

<a> Consumable Material necessary to close the drain holes:

Pressure Sensitive

Tape

05RFB1 As required

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 37

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

Laminating ResinEpoxy Srm Type 2 -

13EBC1 As required

Methyl-Ethyl-Ketone 08BBF1 As required

Trichloroethane

Legacy

08BBU9 As required

5 Do repetitive thermography inspections until the repair of the affected area

has been done, refer to NTM 51-10-25 (preferred) or refer to NTM Task

55-40-50-290-801.

NOTE: In case of any findings during the pulse thermography

inspection, save the images and send it together with the

report sheet to AIRBUS.

6 Do the repair in accordance with the SRM.

Due to the pending availability of the SRM improved repair, contact AIRBUS

for detailed repair instructions.

7 Report the repair to AIRBUS. Use the report sheet Fig. A-GBHAA Sheet 02.

8 If more than 5 local single spots per side shell larger than 1500 mm2 (2.33

sq.in.) and up to 5000 mm2 (7.75 sq.in.) have been detected, report to

AIRBUS and follow their instructions. Use the report sheet Fig. A-GBHAA

Sheet 01.

9 If local single spots larger than 5000 mm2 (7.75 sq.in.) with fluid ingress have

been detected, report the findings to AIRBUS and follow their instructions. Use

the report sheet Fig. A-GBHAA Sheet 01.

(5) Subtask 555007-832-205-001 - Do the ELCH and/or UT inspection around identified

repairs/fluid ingress

Manpower Resources

Manhours 0

Minimum number of person 1

Subtask elapsed time 0

Skills NON DESTRUCTIVE

TESTING

Material necessary to do the job

Consumable CMLD01

ITEM DESCRIPTION REFERENCE TO

CML MAT. No.

QTY PER A/C SEE

NOTES

Non Aqueous CleanerGeneral08BAA9 As required

Textile-Lint Free Cotton 14SBA1 As required

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 38

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

References

Non Destructive Test Manual (NTM) 51-10-24

51-10-26

55-40-09 Para 2.C

Fig. A-GBEAA

Typical pulse thermography and

ELCH/UT inspection

Sheet 01

Sheet 02 - Repair size assessment

Sheet 03 - Repair size assessment

Sheet 04 - Boundary and grid of ELCH/UT

inspections

Sheet 05 - ELCH inspection grid

Fig. A-GBGAA

Rudder skin thickness identification

Sheet 01

Sheet 02

Sheet 03

Fig. A-GBHAA

Report sheet and sketches

Sheet 01 - Pulse thermography report sheet

Sheet 02 - Repair records report sheet

Sheet 03

Sheet 04

(a) If necessary, clean the areas to be inspected with:

Non Aqueous

Cleaner-General

08BAA9 As required

and

Textile-Lint Free

Cotton

14SBA1 As required

(b) Identify the skin thickness of the areas to be inspected, refer to Fig. A-GBGAA

Sheet 02 and Fig. A-GBGAA Sheet 03.

(c) If the skin thickness of the affected areas does not exceed 1.5 mm (0.06 in.), do an

ELCH inspection around the marked repair areas, refer to NTM 51-10-26.

1 For the ELCH inspection, use a grid of 75 mm x 75 mm from the boundary of

the largest repair ply up to 200 mm around the largest repair ply, refer to Fig.

A-GBEAA Sheet 04.

a For the adjustment of the ELCH, refer to NTM 51-10-26.

b For the assessment criteria (yellow and red values) for the ELCH

inspection, refer to NTM 55-40-09 Para 2.C.

(d) If the skin of the affected areas is thicker than 1.5 mm (0.06 in.), do an UT

inspection around the marked repair areas, refer to NTM 51-10-24.

1 Do the UT inspection in an area between the boundary of the largest repair

ply up to 75 mm around the largest repair ply, refer to Fig. A-GBEAA Sheet

04.

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 39

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

(e) If a damage has been detected during the ELCH/UT inspection, provide detailed

information of the identified repair, report to AIRBUS and follow their instructions.

Use the report sheet Fig. A-GBHAA Sheet 02 and the rudder related sketches,

refer to Fig. A-GBHAA Sheet 03 and Fig. A-GBHAA Sheet 04.

(f) If no damage has been detected during the ELCH/UT inspection, continue with the

steps given in the Subtask 555007-832-206-001 of this Service Bulletin.

(6) Subtask 555007-832-206-001 - Do terminating actions in case of no damage

detected

Manpower Resources

Manhours 0

Minimum number of person 1

Subtask elapsed time 0

Skills NON DESTRUCTIVE

TESTING

Material necessary to do the job

Consumable CMLD01

ITEM DESCRIPTION REFERENCE TO

CML MAT. No.

QTY PER A/C SEE

NOTES

Adhesive Film TapeAluminium Foil05RAB9 As required

Pressure Sensitive Tape 05RFB1 As required

Self-Adhes. Disks 05TNB1 As required

Methyl-Ethyl-Ketone 08BBF1 As required

Trichloroethane Legacy 08BBU9 As required

Laminating Resin-Epoxy

Srm Type 2 -

13EBC1 As required

References

Fig. A-GBFAA

Core ventilation procedure

Sheet 01

Sheet 02

Sheet 03

Fig. A-GBHAA

Report sheet and sketches

Sheet 01 - Pulse thermography report sheet

Sheet 02 - Repair records report sheet

Sheet 03

Sheet 04

Fig. A-GFAAA

Flow Chart

Sheet 01 - Flow Chart 1

Sheet 02 - Flow Chart 2

Sheet 03 - Flow Chart 3

Sheet 04 - Flow Chart 4

Sheet 05 - Flow Chart 5

Sheet 06

Fig. A-GAAAA

Closing of ventilation holes

Sheet 01

Sheet 02

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 40

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

(a) If no damage has been detected, continue with the subsequent work steps in

accordance with the Flow Chart Fig. A-GFAAA Sheet 02:

1 If a repair up to 10000 mm2 (15.50 sq.in.) has been detected, provide detailed

information about the repair and report to AIRBUS. Use the report sheet Fig.

A-GBHAA Sheet 02 and the rudder related sketches, refer to Fig. A-GBHAA

Sheet 03 and Fig. A-GBHAA Sheet 04.

2 If a repair larger than 10000 mm2 (15.50 sq.in.) and up to 20000 mm2 (31.00

sq.in.) has been detected, do the ventilation of the core:

NOTE: Instead of the core ventilation procedure, you can do repetitive

ELCH and/or UT inspections around the repair areas until the

repair has been done, refer to Subtask 555007-832-205-001.

a

CAUTION: TO DRILL THE HOLES APPLY MODERATE

PRESSURE TO PREVENT DAMAGE TO THE SKIN, AT

THE END OF THE DRILLING OPERATION. DO NOT

DRILL THE OPPOSITE SHELL.

Drill the holes to a DIA of 3.0 mm (0.12 in.) through the outer and inner

skin in accordance with the dimensions shown on Fig. A-GBFAA Sheet

02 and Fig. A-GBFAA Sheet 03.

NOTE: Repairs behind the trailing edge screw line must not be

vented.

b Temporary restoration of the drain holes option 1:

<1> Close the drain holes with:

Adhesive Film

Tape- Aluminium

Foil

05RAB9 As required

or

Self-Adhes. Disks 05TNB1 As required

<2> Do repetitive detailed inspections of the restored area for loose or

lost adhesive disks or tape until the repair of the affected area has

been done.

<3> In case of loose or lost tape or disks, close the holes again with:

Adhesive Film

Tape- Aluminium

Foil

05RAB9 As required

or

Self-Adhes. Disks 05TNB1 As required

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 41

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

c Temporary restoration of the drain holes option 2:

<1> Close the drain holes in accordance with the instructions given in

the Figure Fig. A-GAAAA Sheet 01 and Fig. A-GAAAA Sheet 02.

<a> Consumable Material necessary to close the drain holes:

Pressure Sensitive

Tape

05RFB1 As required

Laminating ResinEpoxy Srm Type 2 -

13EBC1 As required

Methyl-Ethyl-Ketone 08BBF1 As required

Trichloroethane

Legacy

08BBU9 As required

d Report the results and the planned terminating action to AIRBUS. Use

the report sheet Fig. A-GBHAA Sheet 02.

e Do the terminating action in accordance with the SRM.

Due to the pending availability of the SRM improved repair, contact

AIRBUS for detailed repair instructions.

NOTE: The new repair cutout is equal to the largest outer skin

repair ply.

3 If a repair larger than 20000 mm2 (31.00 sq.in.) and up to 80000 mm2 (124

sq.in.) has been detected, do the ventilation of the core:

a

CAUTION: TO DRILL THE HOLES APPLY MODERATE

PRESSURE TO PREVENT DAMAGE TO THE SKIN, AT

THE END OF THE DRILLING OPERATION. DO NOT

DRILL THE OPPOSITE SHELL.

Drill the holes to a DIA of 3.0 mm (0.12 in.) through the outer and inner

skin in accordance with the dimensions shown on Fig. A-GBFAA Sheet

02 and Fig. A-GBFAA Sheet 03.

b Temporary restoration of the drain holes option 1:

<1> Close the drain holes with:

Adhesive Film

Tape- Aluminium

Foil

05RAB9 As required

or

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 42

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

Self-Adhes. Disks 05TNB1 As required

<2> Do repetitive detailed inspections of the restored area for loose or

lost adhesive disks or tape until the repair of the affected area has

been done.

<3> In case of loose or lost tape or disks, close the holes again with:

Adhesive Film

Tape- Aluminium

Foil

05RAB9 As required

or

Self-Adhes. Disks 05TNB1 As required

c Temporary restoration of the drain holes option 2:

<1> Close the drain holes in accordance with the instructions given in

the Figure Fig. A-GAAAA Sheet 01 and Fig. A-GAAAA Sheet 02.

<a> Consumable Material necessary to close the drain holes:

Pressure Sensitive

Tape

05RFB1 As required

Laminating ResinEpoxy Srm Type 2 -13EBC1 As required

Methyl-Ethyl-Ketone 08BBF1 As required

Trichloroethane

Legacy

08BBU9 As required

d Report the results and the planned terminating action to AIRBUS. Use

the report sheet Fig. A-GBHAA Sheet 02.

e Do the terminating action in accordance with the SRM.

NOTE: The new repair cutout is equal to the largest outer skin

repair ply.

NOTE: If the repair is larger than 30000 mm2 (46.50 sq.in.),

contact AIRBUS for additional instructions.

4 If a repair larger than 80000 mm2 (124 sq.in.) has been detected, do the

ventilation of the core:

a

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 43

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

CAUTION: TO DRILL THE HOLES APPLY MODERATE

PRESSURE TO PREVENT DAMAGE TO THE SKIN, AT

THE END OF THE DRILLING OPERATION. DO NOT

DRILL THE OPPOSITE SHELL.

Drill the holes to a DIA of 3.0 mm (0.12 in.) through the outer and inner

skin in accordance with the dimensions shown on Fig. A-GBFAA Sheet

02 and Fig. A-GBFAA Sheet 03.

b Temporary restoration of the drain holes option 1:

<1> Close the drain holes with:

Adhesive Film

Tape- Aluminium

Foil

05RAB9 As required

or

Self-Adhes. Disks 05TNB1 As required

<2> Do repetitive detailed inspections of the restored area for loose or

lost adhesive disks or tape until the repair of the affected area has

been done.

<3> In case of loose or lost tape or disks, close the holes again with:

Adhesive Film

Tape- Aluminium

Foil

05RAB9 As required

or

Self-Adhes. Disks 05TNB1 As required

c Temporary restoration of the drain holes option 2:

<1> Close the drain holes in accordance with the instructions given in

the Figure Fig. A-GAAAA Sheet 01 and Fig. A-GAAAA Sheet 02.

<a> Consumable Material necessary to close the drain holes:

Pressure Sensitive

Tape

05RFB1 As required

Laminating ResinEpoxy Srm Type 2 -13EBC1 As required

Methyl-Ethyl-Ketone 08BBF1 As required

Trichloroethane

Legacy

08BBU9 As required

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 44

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

d Report the results and the planned terminating action to AIRBUS. Use

the report sheet Fig. A-GBHAA Sheet 02.

e Do the terminating action:

Replace the rudder in accordance with the grace period given in the

accomplishment timescale table

or

replace the affected rudder shell.

NOTE: The rudder shell replacement can be done only at

the AIRBUS Stade facility. Before sending the rudder,

contact:

AIRBUS

Department SBO5 Monitored Retrofit Campaign Account

MONITORED.RETROFIT@airbus.com

to validate the feasibility of the rudder shell replacement.

No further action is necessary in accordance with this Service Bulletin.

(7) Subtask 555007-832-207-001 - Inspect the rudder side shell upper GFRP areas

Manpower Resources

Manhours 0

Minimum number of person 1

Subtask elapsed time 0

Skills NON DESTRUCTIVE

TESTING

Material necessary to do the job

Consumable CMLD01

ITEM DESCRIPTION REFERENCE TO

CML MAT. No.

QTY PER A/C SEE

NOTES

Non Aqueous CleanerGeneral08BAA9 As required

Textile-Lint Free Cotton 14SBA1 As required

References

Non Destructive Test Manual (NTM) Task 51-10-03-280-801

Task 51-10-19-280-801

Task 55-40-50-290-801

Structural Repair Manual (SRM) 51-75-11

51-75-12

Fig. A-GBBAA

Repair type identification

Sheet 01

Sheet 02

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 45

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

References

Fig. A-GFAAA

Flow Chart

Sheet 01 - Flow Chart 1

Sheet 02 - Flow Chart 2

Sheet 03 - Flow Chart 3

Sheet 04 - Flow Chart 4

Sheet 05 - Flow Chart 5

Sheet 06

Fig. A-GBEAA

Typical pulse thermography and

ELCH/UT inspection

Sheet 01

Sheet 02 - Repair size assessment

Sheet 03 - Repair size assessment

Sheet 04 - Boundary and grid of ELCH/UT

inspections

Sheet 05 - ELCH inspection grid

Fig. A-GABAA

Paint borer instructions

Sheet 01

Sheet 02

Sheet 03

Sheet 04

Sheet 05

Sheet 06

Sheet 07

Sheet 08

(a) If repairs in the rudder side shell upper GFRP area are recorded, do the

subsequent inspections in accordance with the Flow Chart Fig. A-GFAAA Sheet 04:

1 Make sure that the paint thickness in the areas to be inspected by pulse

thermography does not exceed:

- 400 microns.

- 400 microns below the decal foil if a decal foil is installed.

NOTE: It is the responsibility of the operator to ensure that the paint

thickness in all areas to be inspected is below or equal to the

limit of 400 microns.

a If the paint coating and/or logo application is too thick, abrade the paint in

accordance with the SRM 51-75-11 to a thickness below or equal to the

limit of 400 microns.

NOTE: Chemical paint stripping is not allowed.

b In case of doubts about the paint thickness, measure the thickness using

a Paint Borer Kit, refer to the Figure Fig. A-GABAA Sheet 01 thru Fig. AGABAA Sheet 08.

<1>

CAUTION: DO NOT DRILL DEEPLY INTO THE BASE

MATERIAL (CFRP OR GFRP). DRILLING TOO

DEEP LEADS TO DAMAGE IN THE OUTER SKIN

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 46

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

If you damage the outer skin with the paint borer, refer to the

Subtask 555007-833-201-001 for repair instructions.

2 Clean the areas to be inspected with:

Non Aqueous

Cleaner-General

08BAA9 As required

and

Textile-Lint Free

Cotton

14SBA1 As required

3 Do a pulse thermography inspection to get the precise location and size of the

repair, refer to NTM Task 55-40-50-290-801.

NOTE: As an alternative for the pulse thermography inspection, you

can identify the repair size by local sanding, refer to Subtask

555007-832-208-001.

NOTE: The pulse thermography inspection indicates the outer skin

repair ply geometry. The largest repair ply defines the

boundary of the repair area.

NOTE: Make sure that you use the pulse thermography inspection

parameters for GFRP, refer to NTM Task 55-40-50-290-801.

4 Mark the boundary of the repair area, refer to Fig. A-GBEAA Sheet 02 and

Fig. A-GBEAA Sheet 03.

5 If a repair type A-A, refer to Fig. A-GBBAA Sheet 02, has been identified, do a

Tap test inspection on the repair, refer to NTM Task 51-10-03-280-801 or

NTM Task 51-10-19-280-801, to identify a skin to core disbonding.

6 For all other repair types, do the ELCH and/or UT inspection around the

repair, refer to the Subtask 555007-832-205-001 of this Service Bulletin.

7 If fluid ingress has been detected, refer to Subtask 555007-832-204-001 of

this Service Bulletin.

8 For further actions continue with the instructions given in the Subtask

555007-832-206-001 and the actions in the Flow Chart Fig. A-GFAAA Sheet

02 of this Service Bulletin.

9 After the inspection, restore the paint coating in accordance with the SRM

51-75-12.

NOTE: Refer to OIT 999.0130/06 ’paint system - best practices’.

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 47

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

(b) If there is no information about repairs in the rudder side shell upper GFRP area,

do the subsequent inspections in accordance with the Flow Chart Fig. A-GFAAA

Sheet 04:

1 Make sure that the paint thickness in the areas to be inspected by pulse

thermography does not exceed:

- 400 microns.

- 400 microns below the decal foil if a decal foil is installed.

NOTE: It is the responsibility of the operator to ensure that the paint

thickness in all areas to be inspected is below or equal to the

limit of 400 microns.

a If the paint coating and/or logo application is too thick, abrade the paint in

accordance with the SRM 51-75-11 to a thickness below or equal to the

limit of 400 microns.

NOTE: Chemical paint stripping is not allowed.

b In case of doubts about the paint thickness, measure the thickness using

a Paint Borer Kit, refer to the Figure Fig. A-GABAA Sheet 01 thru Fig. AGABAA Sheet 08.

<1>

CAUTION: DO NOT DRILL DEEPLY INTO THE BASE

MATERIAL (CFRP OR GFRP). DRILLING TOO

DEEP LEADS TO DAMAGE IN THE OUTER SKIN

If you damage the outer skin with the paint borer, refer to the

Subtask 555007-833-201-001 for repair instructions.

2 Clean the areas to be inspected with:

Non Aqueous

Cleaner-General

08BAA9 As required

and

Textile-Lint Free

Cotton

14SBA1 As required

3 Do a pulse thermography inspection on the complete GFRP area to identify

repairs, refer to NTM Task 55-40-50-290-801.

NOTE: The pulse thermography inspection indicates the outer skin

repair ply geometry. The largest repair ply defines the

boundary of the repair area.

NOTE: Make sure that you use the pulse thermography inspection

parameters for GFRP, refer to NTM Task 55-40-50-290-801.

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 48

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

4 If repairs which are not manufacturing rework have been identified, mark the

boundary of the repair area, refer to Fig. A-GBEAA Sheet 02 and Fig. AGBEAA Sheet 03.

5 Do a Tap test inspection, refer to NTM Task 51-10-03-280-801 or NTM Task

51-10-19-280-801, on the complete GFRP area to identify a skin to core

disbonding.

6 Do the ELCH and/or UT inspection around the repair, refer to the Subtask

555007-832-205-001 of this Service Bulletin.

7 If fluid ingress has been detected, refer to Subtask 555007-832-204-001 of

this Service Bulletin.

8 For further actions continue with the instructions given in the Subtask

555007-832-206-001 and the actions in Flow Chart Fig. A-GFAAA Sheet 02 of

this Service Bulletin.

9 After the inspection, restore the paint coating in accordance with the SRM

51-75-12.

NOTE: Refer to OIT 999.0130/06 ’paint system - best practices’.

(8) Subtask 555007-833-201-001 - Close the holes in case of drilling thru the outer

skin during paint thickness measurement

Manpower Resources

Manhours 0

Minimum number of person 1

Subtask elapsed time 0

Skills NON SPECIFIC

Material necessary to do the job

Consumable CMLD01

ITEM DESCRIPTION REFERENCE TO

CML MAT. No.

QTY PER A/C SEE

NOTES

Adhesive Film TapeAluminium Foil05RAB9 As required

Self-Adhes. Disks 05TNB1 As required

Non Aqueous CleanerGeneral08BAA9 As required

Laminating Resin-Epoxy

Srm Type 2 -

13EBC1 As required

Textile-Lint Free Cotton 14SBA1 As required

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 49

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

References

Structural Repair Manual (SRM) 51-75-12

51-77-10 Para 5

51-77-11 Para 4.M.(2)

51-77-11 Para 4.A.(3)

51-77-11 Para 4.E

51-77-11 Para 5.D

51-77-11 Figure 14

(a) Hole closing procedure option 1:

1

WARNING: OBEY THE MANUFACTURER’S INSTRUCTIONS WHEN

YOU USE CLEANING AGENTS, ADHESIVES, SEALANTS

AND PAINTS: THESE MATERIALS ARE DANGEROUS.

WARNING: WEAR THE CORRECT PROTECTIVE GLOVES, GOGGLES

AND FILTER MASKS WHEN YOU USE CLEANING AGENTS,

ADHESIVES, SEALANTS AND PAINTS: THESE MATERIALS

ARE DANGEROUS.

Prepare and dry the restoration area in accordance with the SRM 51-77-11

Para 4.M.(2).

2 Prepare in accordance with the SRM 51-77-11 Para 4.A.(3):

Laminating ResinEpoxy Srm Type 2 -13EBC1 As required

NOTE: The data sheets for each adhesive, resin or low density

compound states the maximum quantity that can be safely

mixed at one time without causing an exotherm reaction.

Always refer to the appropriate data sheet before mixing the

chosen material.

3 Warm up the mixed resin to a maximum temperature of 45 ̊C (113 F).

4 Put the resin in a syringe volume 10 ml with a needle DIA 1.0 mm (0.04 in.)

and inject the resin through the hole into the cells of the honeycomb core.

Start the injection at the cell bottom and finish when the resin is leaking out of

the hole.

5 Close the filled holes with

Adhesive Film

Tape- Aluminium

Foil

05RAB9 As required

or

Self-Adhes. Disks 05TNB1 As required

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 50

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

6 Let the resin cure for a minimum of 6 hours at room temperature.

If the room temperature is below 18 ̊C (64F), extend the curing time and

perform a gelation test outside the restoration area. After resin gelation plus 2

h, the aircraft can be released to operations again.

OR

Cure the resin at 60 ̊C (140F) for 45 minutes. Install a heating blanket with a

vacuum bag on the rudder surface in accordance with the SRM 51-77-11 Para

5.D, and control the temperature by means of thermocouples in accordance

with the SRM 51-77-11 Figure 14.

7 Do the final surface restoration in accordance with the compliance time given

in Para 1.E.(2), table 5:

a Remove the self adhesive tape from the restoration areas.

b Inspect the restoration in accordance with the SRM 51-77-10 Para 5.

c Remove any surplus resin from the border area of the restoration. Use

abrasive cloth. Start with 280 grade and finish with 400 grade.

d Clean the restoration areas in accordance with the SRM 51-77-11 Para

4.E. Use:

Non Aqueous

Cleaner-General

08BAA9 As required

and

Textile-Lint Free

Cotton

14SBA1 As required

e Restore the surface protection in accordance with the SRM 51-75-12.

(b) Hole closing procedure option 2:

1

WARNING: OBEY THE MANUFACTURER’S INSTRUCTIONS WHEN

YOU USE CLEANING AGENTS, ADHESIVES, SEALANTS

AND PAINTS: THESE MATERIALS ARE DANGEROUS.

WARNING: WEAR THE CORRECT PROTECTIVE GLOVES, GOGGLES

AND FILTER MASKS WHEN YOU USE CLEANING AGENTS,

ADHESIVES, SEALANTS AND PAINTS: THESE MATERIALS

ARE DANGEROUS.

Prepare and dry the restoration area in accordance with the SRM 51-77-11

Para 4.M.(2).

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 51

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

2 Prepare in accordance with the SRM 51-77-11 Para 4.A.(3):

Laminating ResinEpoxy Srm Type 2 -13EBC1 As required

NOTE: The data sheets for each adhesive, resin or low density

compound states the maximum quantity that can be safely

mixed at one time without causing an exotherm reaction.

Always refer to the appropriate data sheet before mixing the

chosen material.

3 Warm up the mixed resin to a maximum temperature of 45 ̊C (113 F).

4 Put the resin in a syringe volume 10 ml with a needle DIA 1.0 mm (0.04 in.)

and inject the resin through the hole into the cells of the honeycomb core.

Start the injection at the cell bottom and finish when the resin is leaking out of

the hole.

5 Close the filled holes with

Adhesive Film

Tape- Aluminium

Foil

05RAB9 As required

or

Self-Adhes. Disks 05TNB1 As required

6 Let the resin cure for a minimum of 12 hours at room temperature.

If the room temperature is below 18 ̊C (64F), extend the curing time and

perform a gelation test outside the restoration area.

After resin gelation plus 4 h, continue with the subsequent steps:

a Remove the self adhesive tape from the restoration areas.

b Inspect the restoration in accordance with the SRM 51-77-10 Para 5.

c Remove any surplus resin from the border area of the restoration. Use

abrasive cloth. Start with 280 grade and finish with 400 grade.

d Clean the restoration areas in accordance with the SRM 51-77-11 Para

4.E. Use:

Non Aqueous

Cleaner-General

08BAA9 As required

and

Textile-Lint Free

Cotton

14SBA1 As required

e Restore the surface protection in accordance with the SRM 51-75-12.

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 52

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

(9) Subtask 555007-832-208-001 - Identify the repair size by local sanding

Manpower Resources

Manhours 0

Minimum number of person 1

Subtask elapsed time 0

Skills AIRFRAME

References

Non Destructive Test Manual (NTM) 55-40-50

Structural Repair Manual (SRM) 51-23-11

51-75-11 Para 3.D

51-75-12

51-77-10

51-77-11 Para 4.D

51-77-11 Para 4.E

51-77-11 Para 4.G

Fig. A-GFAAA

Flow Chart

Sheet 01 - Flow Chart 1

Sheet 02 - Flow Chart 2

Sheet 03 - Flow Chart 3

Sheet 04 - Flow Chart 4

Sheet 05 - Flow Chart 5

Sheet 06

Fig. A-GBDAA

Booster area definition

Sheet 01

Sheet 02

Sheet 03

Fig. A-GBHAA

Report sheet and sketches

Sheet 01 - Pulse thermography report sheet

Sheet 02 - Repair records report sheet

Sheet 03

Sheet 04

Fig. A-GBEAA

Typical pulse thermography and

ELCH/UT inspection

Sheet 01

Sheet 02 - Repair size assessment

Sheet 03 - Repair size assessment

Sheet 04 - Boundary and grid of ELCH/UT

inspections

Sheet 05 - ELCH inspection grid

CAUTION: IT IS THE OPERATOR’S RESPONSIBILITY TO ENSURE THAT

STRUCTURAL SIDE SHELL OUTER SKIN PLY (CFRP OR GFRP) IN

ACCORDANCE WITH THE DESIGN DRAWING IS NOT DAMAGED

DURING THE LOCAL SANDING PROCESS.

REMARK: IN MOST OF THE RUDDER SURFACE THE OUTER

SKIN CONSISTS ONLY OF ONE CFRP OR GFRP PLY. IN

CASE OF SANDING DAMAGE IMMEDIATE REPAIR BEFORE NEXT

FLIGHT IS REQUIRED. AN AREA DAMAGED BY THE LOCAL

SANDING COMBINED WITH AN EXISTING REPAIR CAN LEAD

TO A NON-REPAIRABLE SIZE AND SUBSEQUENT SIDE SHELL

REPLACEMENT.

NOTE: The local sanding procedure is only valid for fully documented repairs.

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 53

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

(a) Do the subsequent work steps in accordance with the Flow Chart Fig. A-GFAAA

Sheet 01, beginning with the box ’LOCAL PAINT THICKNESS IDENTIFICATION’.

1 Identify the paint thickness and the initial basic primer on top of the repair and

beside the repair location.

NOTE: It is recommended to use a Paint Borer Kit Model 518, 518S

or 518MC.

2 Clean the previous repair area in accordance with the SRM 51-77-11 Para

4.E.

3 Do a local mechanical sanding on top and around the repair in accordance

with the SRM 51-75-11 Para 3.D on a step-by-step basis up to the initial basic

primer layer.

NOTE: The allowed maximum repair size is 1m2 (10.76sq.ft.) per local

repair.

4 If the largest repair ply is visible:

a Remove the dust and dry the area in accordance with the SRM 51-77-11

Para 4.G.

b Use a magnifying lens to inspect the sanded area for damage.

<1> In case of findings, do the damage assessment in accordance with

the SRM 51-77-10.

c Mark the boundary of the repair area, refer to Fig. A-GBEAA Sheet 02

and Fig. A-GBEAA Sheet 03.

d Identify the booster areas in accordance with Fig. A-GBDAA Sheet 02

and Fig. A-GBDAA Sheet 03.

e If repairs in the booster areas up to 55000 mm2 (85.25 sq.in.) have

been detected, report the findings to AIRBUS. Use the report sheet Fig.

A-GBHAA Sheet 02 and the rudder related sketches, refer to Fig. AGBHAA Sheet 03 and Fig. A-GBHAA Sheet 04.

<1> Restore the surface protection in accordance with the SRM

51-23-11.

No further actions on these repairs in accordance with this Service

Bulletin.

f If repairs in the booster areas larger than 55000 mm2 (85.25 sq.in.) have

been detected, do the UT inspection around the repair in accordance with

Subtask 555007-832-205-001 of this Service Bulletin.

g If repairs not in the booster area have been detected, do the ELCH

and/or UT inspection in accordance with Subtask 555007-832-205-001 of

this Service Bulletin.

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 54

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

h If fluid ingress has been detected during the pulse thermography

inspection, refer to Subtask 555007-832-204-001 of this Service Bulletin.

i After the inspection, restore the paint coating in accordance with the

SRM 51-75-12 and SRM 51-23-11.

NOTE: Refer to OIT 999.0130/06 ’paint system - best practices’.

5 If the largest repair ply is not visible, continue the local mechanical sanding on

top and around the repair in accordance with the SRM 51-77-11 Para 4.D

on a step-by-step basis up to the pore filler or adhesive with a radius of

approximately 50.0mm (1.97in.) beyond the initial detected repair patch.

6 If the largest repair ply is visible now:

a Remove the dust and dry the area in accordance with the SRM 51-77-11

Para 4.G.

b Mark the boundary of the repair area, refer to Fig. A-GBEAA Sheet 02

and Fig. A-GBEAA Sheet 03.

c Use a magnifying lens to inspect the sanded area for damage.

d In case of findings, do the damage assessment in accordance with the

SRM 51-77-10.

e Identify the booster areas in accordance with Fig. A-GBDAA Sheet 02

and Fig. A-GBDAA Sheet 03.

f If repairs in the booster areas up to 55000 mm2 (85.25 sq.in.) have

been detected, report the findings to AIRBUS. Use the report sheet Fig.

A-GBHAA Sheet 02 and the rudder related sketches, refer to Fig. AGBHAA Sheet 03 and Fig. A-GBHAA Sheet 04.

<1> Restore the surface protection in accordance with the SRM

51-23-11.

No further actions on these repairs in accordance with this Service

Bulletin.

g If repairs in the booster areas larger than 55000 mm2 (85.25 sq.in.) have

been detected, do the UT inspection around the repair in accordance with

Subtask 555007-832-205-001 of this Service Bulletin.

h If repairs not in the booster area have been detected, do the ELCH

and/or UT inspection in accordance with Subtask 555007-832-205-001 of

this Service Bulletin.

i If fluid ingress has been detected during the pulse thermography

inspection, refer to Subtask 555007-832-204-001 of this Service Bulletin.

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 55

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

j After the inspection, restore the paint coating in accordance with the

SRM 51-75-12 and SRM 51-23-11.

NOTE: Refer to OIT 999.0130/06 ’paint system - best practices’.

7 If the largest repair ply is still not visible:

a Remove the dust and dry the area in accordance with the SRM 51-77-11

Para 4.G.

b Do a pulse thermography inspection to get the precise location and the

size of the repair, refer to NTM 55-40-50.

NOTE: The pulse thermography inspection indicates the outer

skin repair ply geometry. The largest repair ply defines

the boundary of the repair area.

NOTE: In case of any findings (repair, damage, fluid ingress)

during the pulse thermography inspection, save the

images and send it together with the report sheet to

AIRBUS.

c Mark the boundary of the repair area, refer to Fig. A-GBEAA Sheet 02

and Fig. A-GBEAA Sheet 03.

d If fluid ingress has been detected during the pulse thermography

inspection, refer to Subtask 555007-832-204-001 of this Service Bulletin.

e Identify the booster areas in accordance with Fig. A-GBDAA Sheet 02

and Fig. A-GBDAA Sheet 03.

f If repairs in the booster areas up to 55000 mm2 (85.25 sq.in.) have

been detected, report the findings to AIRBUS. Use the report sheet Fig.

A-GBHAA Sheet 02 and the rudder related sketches, refer to Fig. AGBHAA Sheet 03 and Fig. A-GBHAA Sheet 04.

<1> Restore the surface protection in accordance with the SRM

51-23-11.

No further actions on these repairs in accordance with this Service

Bulletin.

g If repairs in the booster areas larger than 55000 mm2 (85.25 sq.in.) have

been detected, do the UT inspection around the repair in accordance with

Subtask 555007-832-205-001 of this Service Bulletin.

h If repairs not in the booster area have been detected, do the ELCH

and/or UT inspection in accordance with Subtask 555007-832-205-001 of

this Service Bulletin.

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 56

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

i After the inspection, restore the paint coating in accordance with the

SRM 51-75-12 and SRM 51-23-11.

NOTE: Refer to OIT 999.0130/06 ’paint system - best practices’.

D. TEST

None

E. CLOSE-UP

(1) Subtask 555007-942-201-001 - Close-up

Manpower Resources

Skills NON SPECIFIC

References

Aircraft Maintenance Manual (AMM) Task 29-00-00-863-801

Task 29-00-00-863-802

Task 29-00-00-863-803

55-40-00, Page Block 601

(a) Make sure that the work areas are clean and clear of tools and other items of

equipment.

(b) Remove the access platforms.

(c) Close the circuit breakers as given in the inspection/check Close-up procedure,

refer to AMM 55-40-00, Page Block 601.

(d) Pressurize the Green Hydraulic System, refer to AMM Task 29-00-00-863-801.

(e) Pressurize the Blue Hydraulic System, refer to AMM Task 29-00-00-863-802.

(f) Pressurize the Yellow Hydraulic System, refer to AMM Task 29-00-00-863-803.

(g) In the cockpit, remove all warning notices.

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 57

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

Z326

MFR

DESCR.

SER. N °

CA CODE

MFG DATE

A/C

PN

NSA9117−63D

XXXXXXXXXXXXX

TS−XXXX

A

B

POSITION OF

RUDDER S/N PLACARD

01

NOTE:

01 USE A MIRROR OR FLEXIBLE ENDOSCOPE IF NECESSARY

B

A

F_SB_555007_6_BAAA_01_02

Figure A-GBAAA - Sheet 01

Rudder SN identification

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 58

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

Z326

A LH SHOWN

RH SIMILAR

A

A

A

B

B

C

C

F

F

E

E

D

D

F_SB_555007_6_BBAA_01_01

Figure A-GBBAA - Sheet 01

Repair type identification

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 59

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

OUTER SKIN WITH CORE CLOSING

OUTER SKIN AND CORE REPAIR

WITHOUT CORE CLOSING

OUTER SKIN AND CORE REPAIR

WITH CORE CLOSING

DELAMINATION AND CORE DAMAGE WITH

CORE CLOSING (SRM 55−41−00 PAGE BLOCK 201 FIG.201/205)

A A

B B

C C

(SRM 55−41−00 PAGE BLOCK 201 FIG.203/207)

(SRM 55−41−00 PAGE BLOCK 201 FIG.204/208/211)

(SRM 55−41−00 PAGE BLOCK 201 FIG.204/208/211)

D D

E E

F F

OUTER SKIN WITHOUT CORE CLOSING

(SRM 55−41−00 PAGE BLOCK 201 FIG. 212)

(SRM 55−41−13 PAGE BLOCK 201 FIG. 203)

EXAMPLES OF POSSIBLE DAMAGE TYPES

(TAKEN FROM THE A340−200/300 SRM PROCEDURES)

(SRM 55−41−00 PAGE BLOCK 201 FIG.204/208/211) (SRM 55−41−00 PAGE BLOCK 201 FIG. 204/208/209/213/214)

(SRM 55−41−13 PAGE BLOCK 201 FIG.204) (SRM 55−41−13 PAGE BLOCK 201 FIG.206)

BOTH SKIN AND CORE REPAIR

WITH AND WITHOUT CORE CLOSING /

REPAIR WITH ACCESS FROM ONE SIDE ONLY

BOTH SKIN AND CORE REPAIR WITH AND WITHOUT 

CORE CLOSING / REPAIR WITH ACCESS FROM BOTH SIDE

F_SB_555007_6_BBAA_02_03

Figure A-GBBAA - Sheet 02

Repair type identification

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 60

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

REPAIR PROCEDURE

202

15.A., 15.C.

55−41−00

TEMPORARY REPAIR FOR LARGE DAMAGE.

55−41−13 5.B.

55−41−00 REPAIR FOR ABRASIONS AND SCRATCHES IN THE RUDDER ZONE "A,B". 11.A., 11.C.

55−41−00 206

55−41−00

5.A.

REPAIR FOR APEX STRIP IN THE RUDDER ZONE "D".

55−41−13 201

202

5.E. 205

REPAIR FOR ABRASIONS AND SCRATCHES IN THE RUDDER ZONE "J".

REPAIR FOR DEBONDING WITHOUT

CRACKS AND HOLES IN RUDDER ZONE "A,E,J,Q AND S".

55−41−00

55−41−13 REPAIR OF EDGE AT LOWER SHELL IN RUDDER ZONE "N".

PARA. FIG.

19.A 210

CHAPTER

TAKEN FROM A340−200/300 SRM ISSUE: 01. OCT 2009

NOTE:

REPAIRS ACCOMPLISHED IN ACCORDANCE WITH THE SRM PROCEDURES GIVEN IN THE LIST ABOVE,

ARE NOT AFFECTED BY THIS SERVICE BULLETIN.

F_SB_555007_6_BCAA_01_03

Figure A-GBCAA - Sheet 01

Repair type identification - SRM list

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 61

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

Z326

A

B

C

A

F_SB_555007_6_BDAA_01_02

Figure A-GBDAA - Sheet 01

Booster area definition

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 62

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

DEFINITION OF

BOOSTER AREA

VALID FOR RUDDER

LH SHOWN

F55471015

B

BR1

BR2

BR3

BR4

BR5

BR6

BR7

BR8A

956.0 mm

(37.64 in)

3188.0 mm

(125.51 in)

995.0 mm

(39.17 in)

F_SB_555007_6_BDAA_02_02

Figure A-GBDAA - Sheet 02

Booster area definition

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 63

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

DEFINITION OF

BOOSTER AREA

VALID FOR RUDDER

RH SHOWN

F55471015

C

BR1

BR2

BR3

BR4

BR5

BR6

BR7

BR8A

956.0 mm

(37.64 in)

3188.0 mm

(125.51 in)

995.0 mm

(39.17 in)

F_SB_555007_6_BDAA_03_02

Figure A-GBDAA - Sheet 03

Booster area definition

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 64

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

Z326

A

A

B E

B E

F_SB_555007_6_BEAA_01_02

Figure A-GBEAA - Sheet 01

Typical pulse thermography and ELCH/UT inspection

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 65

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

TYPICAL 

PULSE THERMOGRAPHY

INSPECTION

LH SHOWN B RH SYMETRICAL

BR1

BR2

BR3

BR4

BR5

BR6

BR7

BR8A

C

D

F_SB_555007_6_BEAA_02_03

Figure A-GBEAA - Sheet 02

Typical pulse thermography and ELCH/UT inspection - Repair size assessment

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 66

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

REPAIR SIZE = D2 x /4

100.0mm x 100.0mm

(3.93 in x 3.93 in)

(15.50 sq.in)

DAMAGE IN THE 

OUTER SKIN AND CORE

MAX. REPAIR PLY

REPAIR PLY

D

 (110.0mm)2 x /4

= (4.33 in2 x /4)

 ca. 10 000 mm2 =

DAMAGE IN THE 

OUTER SKIN AND CORE

MAX. REPAIR PLY

REPAIR PLIES

REPAIR SIZE = A x B

=

50.0mm x 200.0mm

(1.97 in x 7.87 in) =

OR

(15.50 sq.in)

10 000 mm2 =

B

A

EXAMPLE:

EXAMPLE:

D = 110.0mm DIA

C

D

02 THE NEW CUTOUT SIZE FOR THE REPAIR IS THE

SIZE OF THE FORMER OUTER SKIN REPAIR PLY.

02

02

F_SB_555007_6_BEAA_03_01

Figure A-GBEAA - Sheet 03

Typical pulse thermography and ELCH/UT inspection - Repair size assessment

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 67

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

TYPICAL 

ELCH/UT

INSPECTION

LH SHOWN

RH SYMETRICAL

INSPECTION AREA

ELCH/UT

SKIN THICKNESS 1.5mm (0.23 in):

A=200.0mm (7.87 in) 

AROUND THE MAX. REPAIR PLY 

ELCH METHOD

GRID = 75.0mm x75.0mm (2.95 in x 2.95 in)

SKIN THICKNESS 1.5mm (0.23 in):

A=75.0mm (2.95 in) 

AROUND THE MAX. REPAIR PLY 

UT−METHOD

E

BR1

BR2

BR3

BR4

BR5

BR6

BR7

BR8A

F

MAX. REPAIR PLY

A

F_SB_555007_6_BEAA_04_03

Figure A-GBEAA - Sheet 04

Typical pulse thermography and ELCH/UT inspection - Boundary and grid of ELCH/UT inspections

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 68

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

TYPICAL TRAILING EDGE

ELCH INSPECTION

NOTE:

DISTANCE FROM EDGE 

F

75.0 mm

(2.95 in)

75.0 mm

(2.95 in)

EXISTING SCREW

75.0 mm

(2.95 in)

75.0 mm

(2.95 in)

75.0 mm

(2.95 in)

01

01

INSPECTION POINT

ELCH TOOL

TYPICAL TRAILING EDGE

ELCH INSPECTION

AROUND REPAIR AREA

75.0 mm

(2.95 in) 75.0 mm

(2.95 in)

MAX. REPAIR PLY

02

02

02 SCREWS AND ELCH TOOL ARE NOT DRAWN TO SCALE F_SB_555007_6_BEAA_05_05

Figure A-GBEAA - Sheet 05

Typical pulse thermography and ELCH/UT inspection - ELCH inspection grid

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 69

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

Z326

A

B

B

A

F_SB_555007_6_BFAA_01_01

Figure A-GBFAA - Sheet 01

Core ventilation procedure

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 70

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

MAX. RECTANGULAR REPAIR SIZE 100.0mm (3.94 in):

DRILL HOLES THRU INNER AND OUTER SKIN.

CAUTION: DO NOT DRILL THE OPPOSITE SHELL.

NOTE:

03

01

MIN. 90.0 mm

(3.54 in)

100.0 mm

(3.94 in)

02 REPAIR SIZE DETECTED BY THERMOGRAPHY

02

APPLICABLE TO MAX. 6 HOLES

IN A ROW

TYPICAL 

CORE VENTING

IF REPAIR SIZE IS LARGER THAN 105 000mm2 (162.75 sq.in.),

CONTACT AIRBUS FOR FURTHER INSTRUCTIONS

MAX. 100.0 mm

(3.94 in)

03

C

DRILL 1 ROW IN THE MID OF THE REPAIR.

IF THE RECTANGULAR REPAIR SIZE IS LARGER THAN

100.0mm (3.94 in), DRILL 2 ROWS 

AS SHOWN IN FIG. A−GBFAA, SHEET 03.

05 CONFIRM BY AN ADDITIONAL INSPECTION THAT THE DRILL

HOLE HAS PENETRATED THE INNER SKIN.

(E.G. BY INSERTING A SUITABLE PIN DEEPER THAN NOMINAL

PANEL THICKNESS, OR BY ILLUMINATION OF THE RUDDER

FROM INSIDE THROUGH A HOLE IN THE SPAR AND VISUAL A A

01

3.0 mm DIA

(0.12 in)

01

OUTER SKIN

INNER SKIN

OPPOSITE SHELL

MAX. REPAIR PLY

02

C D

A 05

A

50.0 mm

(1.97 in)

TE−SCREW

B

MAX. REPAIR PLY

INSPECTION THROUGH THE DRILL HOLE.) F_SB_555007_6_BFAA_02_04

Figure A-GBFAA - Sheet 02

Core ventilation procedure

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 71

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

IF THE RECTANGULAR REPAIR SIZE IS LARGER THAN

100.0 mm

(3.94 in)

NOTE:

04

MIN. 90.0 mm

(3.54 in) MIN. 90.0 mm (3.54 in)

100.0 mm

(3.94 in)

02 REPAIR SIZE DETECTED BY THERMOGRAPHY

MAX. REPAIR PLY

02

04

D

APPLICABLE TO MAX. 6 HOLES

IN A SQUARE GRID

IF REPAIR SIZE IS LARGER THAN 105 000mm2 (162.75 sq.in.),

CONTACT AIRBUS FOR FURTHER INSTRUCTIONS

> 100.0 mm

(3.94 in)

100.0 mm (3.94 in), DRILL 2 ROWS.

F_SB_555007_6_BFAA_03_00

Figure A-GBFAA - Sheet 03

Core ventilation procedure

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 72

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

Z326

A

B

C

A

F_SB_555007_6_BGAA_01_02

Figure A-GBGAA - Sheet 01

Rudder skin thickness identification

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 73

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

< 1.5mm (0.059 in)

VALID FOR RUDDER

LH SHOWN

SKIN THICKNESS 

> 1.5mm (0.059 in)

SKIN THICKNESS NO INSPECTION

BR1

BR2

BR3

BR4

BR5

BR6

BR7

BR8A

1

F55471015

B

F_SB_555007_6_BGAA_02_02

Figure A-GBGAA - Sheet 02

Rudder skin thickness identification

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 74

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

< 1.5mm (0.059 in)

VALID FOR RUDDER

RH SHOWN

SKIN THICKNESS 

> 1.5mm (0.059 in)

SKIN THICKNESS NO INSPECTION

BR1

BR2

BR3

BR4

BR5

BR6

BR7

BR8A

1

F55471015

C

F_SB_555007_6_BGAA_03_02

Figure A-GBGAA - Sheet 03

Rudder skin thickness identification

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 75

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

REPAIR DETECTED WITH NIL DAMAGE

NO REPAIR DETECTED

PLEASE SEND REPORTING SHEET TO:

AIRBUS

CUSTOMER SERVICE STRUCTURE ENGINEERING

DEPARTMENT SEES2

1 ROND POINT MAURICE BELLONTE

31707 BLAGNAC CEDEX

FRANCE

FAX +33 (0)5 61 93 36 14

Structure.sbinspectionresult@airbus.com

REPAIR DETECTED WITH DAMAGE

PLEASE SEND REPORTING SHEET TO:

DEPARTMENT SEOE1/2/3

NOTE: ATTACH ALSO THE INITIAL PUSLE THERMOGRAPHY PHOTOS.

PREVIOUS REPORTS PER SB55−5007 REV00 FIGURE A−GBHAA − SHEET 01/02/03 ARE VALID

AIRCRAFT

MSN

RUDDER S/N

INSPECTION DATE

FLIGHT CYCLES FC

FLIGHT HOURS FH

DATA

PULSE THERMOGRAPHY

COMPLETE INSPECTION LH AND RH SIDE

YES/NO

INSPECTION RESULT

REPAIR DETECTED

LH

RH

LIQUID INGRESS DETECTION

DAMAGE CHECK UT − ELCH INDICATION

SUMMARY

RUDDER SIDE SHELLS SANDWICH REPAIR PULSE THERMOGRAPHY REPORT

F_SB_555007_6_BHAA_01_04

Figure A-GBHAA - Sheet 01

Report sheet and sketches - Pulse thermography report sheet

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 76

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

PLEASE SEND REPORTING SHEET TO:

AIRBUS

CUSTOMER SERVICE STRUCTURE ENGINEERING

DEPARTMENT SEES2

1 ROND POINT MAURICE BELLONTE

31707 BLAGNAC CEDEX

FRANCE

FAX +33 (0)5 61 93 36 14

Structure.sbinspectionresult@airbus.com

FIGURE A−GBHAA − SHEET 01 / REPORT SHEET AND SKETCHES − REPORT SHEET

PREVIOUS REPORTS PER SB55−5007 REV00 FIGURE A−GBHAA − SHEET 01 ARE VALID

AIRCRAFT

MSN

RUDDER S/N

RECORDS REVIEW DATE

DATA

RECORDS STATUS

REPAIR RECORDS COMPLETE SINCE ORIGINAL

YES/NO

REPAIR SCHEME

RUDDER FLIGHT CYCLES / FLIGHT HOURS

REPAIR DATE

LH OR RH SIDE SHELL

SRM FIGURE 2XX (SRM 55−41−00 AND/OR 55−41−13 PB201)

DAMAGE SIZE (CIRCULAR) DIAMETER IN mm

SUMMARY

RUDDER SIDE SHELLS SANDWICH REPAIR RECORDS

SRM (STRUCTURAL REPAIR MANUAL) REPAIR PERFORMED

REPAIR APPROVED BY LOCAL AIRWORTHINESS

DAMAGE SIZE (RECTANGULAR SHAPE) LENGTH AND WIDTH IN mm

DAMAGE SIZE (mm2)

REPAIR OUTER PLY SIZE (mm2) IF KNOWN FROM RECORDS

LOCATION AS PER SRM 55−41−00 PB101 FIGURE 103 ZONE CODE.

SERVICE BULLETIN NO.: A330−55−5007 REVXX

IN CASE OF MORE THAN 1 REPAIR, DUPLICATE THIS REPORTING SHEET

(0 FLIGHT CYCLES) EIS ENTRY INTO SERVICE

AUTHORITIES (NO AIRBUS APPROVAL)

F_SB_555007_6_BHAA_02_04

Figure A-GBHAA - Sheet 02

Report sheet and sketches - Repair records report sheet

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 77

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

Rudder Side Shell 

(Show damage location, size and type.)

Sandwich Repair Inspection

F55471015

Damage 

location

Damage 

description / type

Damage 

size mm2 / sq.in.

Valid for rudder:

NOTE:

01 FOR THE DAMAGE LOCATION, MARK THE AREA AND IDENTIFY WITH A NUMBER.

01

LH

BR1

BR2

BR3

BR4

BR5

BR6

BR7

BR8A

F_SB_555007_6_BHAA_03_03

Figure A-GBHAA - Sheet 03

Report sheet and sketches

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 78

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

Rudder Side Shell 

(Show damage location, size and type.)

Sandwich Repair Inspection

Damage 

location

Damage 

description / type

Damage 

size mm2 / sq.in.

Valid for rudder:

NOTE:

01 FOR THE DAMAGE LOCATION, MARK THE AREA AND IDENTIFY WITH A NUMBER.

01

RH

F55471015

BR1

BR2

BR3

BR4

BR5

BR6

BR7

BR8A

F_SB_555007_6_BHAA_04_01

Figure A-GBHAA - Sheet 04

Report sheet and sketches

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 79

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

Z326

A

B

B

A

F_SB_555007_6_BJAA_01_02

Figure A-GBJAA - Sheet 01

GFRP area location

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 80

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

VALID FOR RUDDER

LH SHOWN

RH SYMMETRICAL

F55471015

B

BR1

BR2

BR3

BR4

BR5

BR6

BR7

GFRP AREA

CFRP AREA

1012.0 mm

(39.84 in)

BR8A

561.0 mm

(22.09 in)

F_SB_555007_6_BJAA_02_02

Figure A-GBJAA - Sheet 02

GFRP area location

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 81

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

CHECK THE RUDDER RECORDS IF REPAIRS

(AIRBUS RAS , SRM AND OTHER ) 

NO YES

PERFORM PULSE THERMOGRAPHY

INSPECTION ON COMPLETE

REPORT THE INFORMATION TO AIRBUS.

01

PERFORMED

SINCE RUDDER EIS ?

REPAIR

DETECTED, WHICH

NO

YES

REPAIR 

YES NO

REPORT THE INFORMATION TO AIRBUS.

PERFORM ELCH AND/OR UT 

AROUND THE IDENTIFIED

NO FURTHER ACTION

REQUIRED IN ACCORDANCE

WITH THIS SB.

REFER TO FLOW CHART 2 FOR 

ACTIONS ON IDENTIFIED REPAIRS.

COMPLETE REPAIR

RECORDS AVAILABLE

SINCE RUDDER EIS ?

REPAIRS.

SIDE SHELLS TO IDENTIFY REPAIRS:

MARK THE REPAIRS.

YES

REPAIRS IN THE BOOSTER

AREA

REPAIR SIZE 55000mm2

03 LARGER THAN

(85.25 sq.in.)

NO

 ARE RECORDED SINCE RUDDER EIS AND

04

05

06

OR NOT IN THE BOOSTER

AREA. 03

REPORT UNDOCUMENTED RUDDER 

S/N LIST TO AIRBUS SEES2 TO GET

RELATED RUDDER MANUFACTURING

REWORK DATA 07

IS NOT MANUFACTURING

REWORK ?

08

12

FOR PAINT THICKNESS IDENTIFICATION

REFER TO FLOW CHART 5

FLUID

NO YES

NO FURTHER 

ACTIONS.

CONTINUE WITH

ACTIONS AS PER

FLOW CHART 3.

INGRESS

DETECTED

REPAIR TYPE

INSPECTED IN ACCORDANCE WITH THE SB.

02 IDENTIFIED TO BE REPORT THE

INFORMATION TO AIRBUS.

PERFORM PULSE THERMOGRAPHY ON REPAIR 

LOCATION TO PRECISE LOCATION AND SIZE.

YES

NO

NO

YES

REPORT THE INFORMATION TO AIRBUS.

MARK THE REPAIRS.

REPAIRS IN THE BOOSTER

AREA

REPAIR SIZE 55000mm2

03 LARGER THAN

(85.25 sq.in.) 06

OR NOT IN THE BOOSTER

AREA. 03

12

FOR PAINT THICKNESS IDENTIFICATION

REFER TO FLOW CHART 5

AND

PERFORM LOCAL SANDING ON TOP AND

REPAIR PLY

OF THE REPAIR

LARGEST 

VISIBLE?

YES

NO

AROUND THE PEPAIR UP TO PRIMER. 28

PERFORM LOCAL SANDING

ON TOP AROUND THE REPAIR

UP TO ADHESIVE. 24 25

REPAIR PLY

OF THE REPAIR

LARGEST 

VISIBLE?

YES

OR

NO

26

LOCAL PAINT THICKNESS IDENTIFICATION 27

MARK REPAIR SIZE ON SURFACE

22 23

25

F_SB_555007_6_FAAA_01_05

Figure A-GFAAA - Sheet 01

Flow Chart - Flow Chart 1

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 82

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

ACTIONS ON IDENTIFIED

REPAIRS

DAMAGE

DETECTED YES NO

PROVIDE DETAILED 

DAMAGE REPORT AND

REPAIR SIZE 

10000mm2, (15.50 sq.in.) −

PROVIDE DETAILED

INFORMATION TO AIRBUS 

AVAILABLE.

PERFORM REPETITIVE 

ELCH AND/OR UT

INSPECTION AROUND THE

IDENTIFIED REPAIR.

PERFORM CORE VENTING

THROUGH INNER SKIN, IN

ACCORDANCE WITH VENTING

SCHEME.

PERFORM CORE VENTING

THROUGH INNER SKIN, IN

ACCORDANCE WITH VENTING

SCHEME.

OR

ON IDENTIFIED REPAIR

DETAILED INFORMATION ON IDENTIFIED REPAIR IF

REPORT TO AIRBUS

AND FOLLOW THEIR

INSTRUCTIONS.

FINDINGS

YES NO

REPORT THE RESULTS AND PLANNED

TERMINATING ACTION ON IDENTIFIED 

REPAIR IN ACCORDANCE WITH

SRM AT THE IDENTIFIED

REPAIR LOCATION.

REPAIR IN ACCORDANCE WITH

SRM AND WITH ADDITIONAL 

INSTRUCTIONS FROM AIRBUS.

REPLACE AFFECTED 

RUDDER SHELL 

OR REPLACE THE RUDDER.

REFER TO FIGURE A−GFAAA, SHEET 06.

NOTE:

09

09 REPAIR SIZE 09 REPAIR SIZE 09 REPAIR SIZE 09

10

10

11

TO AIRBUS SEOE 1/2/3 OR

TERMINATING ACTION

10000mm2, (15.50 sq.in.). 20000mm2, (31.00 sq.in.). 20000mm2, (31.00 sq.in.) − 80000mm2, (124.00 sq.in.). 80000mm2, (124.00 sq.in.).

NO FURTHER ACTION

REQUIRED IN ACCORDANCE

WITH THIS SB.

AIRTAC AND FOLLOW

PERFORM CORE VENTING

THROUGH INNER SKIN, IN

ACCORDANCE WITH VENTING

SCHEME.

REPAIR TO AIRBUS SBO 5, COPY SEES2

REPORT THE RESULTS AND PLANNED

TERMINATING ACTION ON IDENTIFIED 

REPORT THE RESULTS AND PLANNED

TERMINATING ACTION ON IDENTIFIED 

TERMINATING ACTION

REPAIR SIZE 30000mm2, (46.50 sq.in.).

REPAIR SIZE 30000mm2, (46.50 sq.in.).

NO FURTHER ACTION

REQUIRED IN ACCORDANCE

REFER TO FIGURE A−GBEAA. WITH THIS SB.

THEIR INSTRUCTIONS

REPAIR TO AIRBUS SBO 5, COPY SEES2 REPAIR TO AIRBUS SBO 5, COPY SEES2

19

19

F_SB_555007_6_FAAA_02_06

Figure A-GFAAA - Sheet 02

Flow Chart - Flow Chart 2

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 83

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

ACTIONS ON DETECTED FLUID INGRESS.

LOCAL SINGLE SPOT FLUID INGRESS

1500 mm2, (2.33 sq.in.) AND 

5000 mm2, (7.75 sq.in.)

LOCAL SINGLE SPOT FLUID INGRESS

1500 mm2, (2.33 sq.in.)

LOCAL SPOT FLUID INGRESS

5000 mm2, (7.75 sq.in.)

DRAIN BY CORE VENTING.

REPORT TO AIRBUS SEOE 1/2/3 OR AIRTAC

AND FOLLOW THEIR INSTRUCTIONS.

REPORT TO

AIRBUS.

NO FURTHER ACTION REQUIRED

IN ACCORDANCE WITH THIS ISB.

REPETITIVE THERMOGRAPHY

RE− INSPECTION.

DO THE REPAIR.

ACTIONS ON DETECTED FLUID INGRESS.

PERFORM ELCH AND/OR UT AROUND THE

IDENTIFIED FLUID INDICATION

DAMAGE

DETECTED YES

NO

THAN 5 SPOTS PER

NO REPORT TO AIRBUS SEOE 1/2/3 OR AIRTAC

AND FOLLOW THEIR INSTRUCTIONS.

MORE

SIDE SHELL YES

NO

DETECTED

THAN 5 SPOTS PER

SIDE SHELL YES

MORE

DETECTED

NO

F_SB_555007_6_FAAA_03_06

Figure A-GFAAA - Sheet 03

Flow Chart - Flow Chart 3

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 84

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

INSPECT THE RUDDER SIDE SHELL

YES KNOWN IN THE NO

PERFORM 

ON REPAIR LOCATION AND 

YES TYPE A−A NO

IN CASE OF FINDINGS,

TAP TEST INSPECTION

OR WOODPECKER

ALL OTHER REPAIR TYPES:

PERFORM ELCH

IDENTIFIED REPAIRS

CONTINUE WITH

ACTIONS IN FLOW CHART 2

UPPER GFRP AREA

GFRP AREA

REPAIRS

PULSE THERMOGRAPHY INSPECTION

MARK THE REPAIR

REPAIR

REPORTED

PERFORM

INSPECTION

AND/OR UT

AROUND THE

PERFORM 

ON THE COMPLETE

PULSE THERMOGRAPHY INSPECTION

GFRP AREA

TAP TEST INSPECTION OR

WOODPECKER INSPECTION

PERFORM

ON THE COMPLETE GFRP AREA

MARK THE REPAIRS

YES CORE DISBONDING

NO

SKIN TO

IDENTIFIED

ALL OTHER REPAIR TYPES:

PERFORM ELCH

IDENTIFIED REPAIRS

AND/OR UT

AROUND THE

NOTE:

18 REFER TO FIGURE A−GFAAA, SHEET 06.

18

WHICH ARE NOT

MANUFACTURING REWORKS

20

21

F_SB_555007_6_FAAA_04_03

Figure A-GFAAA - Sheet 04

Flow Chart - Flow Chart 4

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 85

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

PULSE THERMOGRAPHY PAINT

OPERATOR

IS SURE THAT THE 

NO

GFRP−AREA

400.00 microns

THICKNESS LIMITATION

RUDDER PAINT THICKNESS

IS BELOW THE GIVEN

LIMITS

YES

APPLY PAINT THICKNESS

MEASUREMENT TOOL

NO

LOCAL PAINT REMOVAL

RUDDER

PAINT THICKNESS

IS BELOW 

THE GIVEN

LIMITS

YES

CONTINUE WITH ACTIONS

DEFINED IN FLOW CHART 1 PAINT RESTORATION IS REQUIRED

AFTER PULSE THERMOGRAPHY

NOTE: AND/OR ELCH/UT INSPECTION

13 REFER TO FIGURE A−FAAA, SHEET 06

13 14

16

15 17

PAINT RESTORATION

IS REQUIRED AFTER

PULSE THERMOGRAPHY

AND/OR ELCH/UT

INSPECTION

CFRP−AREA

800.00 microns

OR

400.00 microns

BELOW DECAL FOIL

F_SB_555007_6_FAAA_05_05

Figure A-GFAAA - Sheet 05

Flow Chart - Flow Chart 5

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 86

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

SEE AIRBUS LIST WITH A/C MSN, RUDDER S/N

SEE AIRBUS DEFINITION OF REPAIR TYPES AFFECTED

BY THE ISB INSPECTION. REFER TO FIGURE A−GBBAA.

SEE AIRBUS BOOSTER DEFINITION. 

NOTE:

01

02

03

AND RAS NUMBER, REFER TO FIGURE A−GBCAA.

IF AN AIRCRAFT LISTED IN THE SB EFFECTIVITY HAS A

REPAIR EMBODIED THAT IS NOT OF AIRBUS ORIGIN, 

04

AND WHICH AFFECTS THE CONTENT OF THIS SB, THE

APPROVAL BY ITS AIRWORTHINESS AUTHORITY FOR

ANY ADAPTATION NECESSARY BEFORE 

THIS ACTION IS NOT NECESSARY, IF THE INFORMATION

HAS BEEN ALREADY SENT TO AIRBUS IN ACCORDANCE

05

NEXT STEP.

REFER TO FIGURE A−GBDAA.

OPERATOR IS RESPONSIBLE FOR OBTAINING THE

INCORPORATION OF THE SB.

WITH THE OIT SE 999.0071/10 CONTINUE WITH THE 

06 REPAIR SIZE DEFINED BY THE LARGEST REPAIR PLY.

07

08 BASED ON PROVIDED AIRBUS EVALUATION OF RUDDER

S/N MANUFACTURING REWORK DATA.

12 FOR GFRP−AREA INSPECTION REFER TO FLOW CHART 4

REPAIR SIZE DEFINED BY THE LARGEST REPAIR PLY.

PENDING AVAILABILITY OF SRM IMPROVED REPAIR, AIRBUS IS TO BE

CONTACTED FOR INSTRUCTIONS.

SIDE SHELL REPLACEMENT CAN BE DONE ONLY AT THE AIRBUS STADE FACILITY.

09

10

11

REFER TO FIGURE A−GBEAA.

19 THE NEW REPAIR CUTOUT IS EQUAL TO

THE LARGEST OUTER SKIN REPAIR PLY.

18 REFER TO FIGURE A−GBBAA

20 IN CASE OF FLUID INGRESS REFER TO

FLOW CHART 3 FOR FURTHER INSTRUCTIONS

21 FOR PAINT THICKNESS IDENTIFICATION REFER TO

FLOW CHART 5

13 PRIOR TO THE APPLICATION OF THE PULSE THERMOGRAPHY

METHOD NTM 55−40−50 THE OPERATOR HAS TO CHECK

THE SIDE SHELL PAINT THICKNESS. IT IS THE 

OPERATORS RESPONSIBILITY TO ENSURE THAT THE

RUDDER SIDE SHELL PAINT THICKNESS IS BELOW THE

GIVEN LIMITS.

PLEASE CONSIDER THE INFORMATION FOR PAINT

RESTORATION PROVIDED WITH THE OIT 999.0130/06

DATED 21 NOV 2006.

SRM 51−75−11 RECOMMENDS ABRADING COMPOSITE

SURFACE UP TO THE FIRST PRIMER COATING IN ORDER

TO AVOID SURFACE DAMAGE OF THE COMPOSITE.

IN CASE OF A SMOOTH AND EVEN PAINT THICKNESS

DISTRIBUTION FIG. A−GABAA PROVIDE GUIDANCE

MATERIAL ABOUT A FEASIBLE PAINT BORER LOCATION 

DISTRIBUTION OVER THE SIDE SHELL.

IN CASE PAINT REMOVAL LARGER THAN 2m2 IS REQUIRED

IT IS RECOMMENDED TO REMOVE THE RUDDER FROM

THE A/C.

14

15

16

17

22 CLEAN THE PREVIOUS REPAIR AREA.

REFER TO SRM 51−77−11 PARA 4.E.

PERFORM A LOCAL MECHANICAL SANDING

A STEP BY STEP BASIS UP TO INITIAL BASIC PRIMER LAYER.

AS PER SRM 51−75−11 PARA 3.D. ON 

23

ON TOP/AROUND THE REPAIR

NO VISIBLE REPAIR: 

USING ABRASIVE CLOTH GRADE 100, 220, 280, 400.

MECHANICAL SANDING ON A STEP BY STEP BASIS

24

CONTINUE LOCAL SANDING UP TO PORE FILLER/ADHESIVE.

REFER TO SRM 51−77−11 PARA 4.D.

25 ENSURE NO DAMAGE TO CFRP OR GFRP BASE MATERIAL.

IF THE LARGEST REPAIR PLY IS NOT VISIBLE,

BEYOUND THE INITIAL DETECTED REPAIR PATCH.

26

CONTINUE LOCAL SANDING ON AND AROUND THE REPAIR WITH A RADIUS APPROX. 50.0mm (1.97in)

27 USE PAINT BORER TO ASSESS LOCAL PAINT SCHEME, THICKNESS AND INITIAL BASIC PRIMER

PRIOR SANDING. USE ON TOP OF REPAIR AND BESIDE REPAIR LOCATION.

28 MAX. 1m2 (10.76 sq.ft.) SANDED AREA PER LOCAL REPAIR IS ALLOWED.

SRM 51−77−10 AND SEND A DETAILED REFERENCE REPORT TO SEOE DEPARTMENT.

IN CASE OF DAMAGE, PERFORM ASSESSMENT AS PER

IT IS THE OPERATOR’S RESPONSIBILITY TO ENSURE THAT THE STRUCTURAL SIDE SHELL OUTER SKIN PLY

(CFRP OR GFRP) IN ACCORDANCE TO THE DESIGN DRAWING IS NOT DAMAGED DURING THE LOCAL 

SANDING PROCESS.

REMARK: IN MOST OF THE RUDDER SURFACE THE OUTER SKIN CONSISTS ONLY OF ONE CFRP OR GFRP PLY!

IN CASE OF SANDING DAMAGE IMMEDIATE REPAIR BEFORE NEXT FLIGHT IS REQUIRED. AN AREA DAMAGED

BY THE LOCAL SANDING COMBINED WITH AN EXISTING REPAIR CAN LEAD TO A NON−REPAIRABLE SIZE

AND SUBSEQUENT SIDE SHELL REPLACEMENT!

REWORK COMPLETE DATA.

AIRBUS MUST BE CONTACTED FOR MANUFACTURING

F_SB_555007_6_FAAA_06_01

Figure A-GFAAA - Sheet 06

Flow Chart

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 87

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

Closing of ventilation holes in outer skin

Method 1 − Application of a bonded cover

NOTE: This repair needs to be re−inspected. Correct cover application has to be ensured by frequent

detailed visual inspection during the application period at intervals not exceeding 900 FH.

1. Apply high speed tape over the ventilation hole, refer to Chapter 51−77−12 Paragraph 2.

Method 2 − Application of laminated cover

NOTE: This repair needs no re−inspection.

2. Prepare the repair area, refer to Chapter 51−77−11 Paragraph 4.M.(2)., apply only step

1 to 2 and 10 to 17.

3. Protect the area adjacent to the repair area with flash tape (Material No. 05RFB1), refer to

Chapter 51−77−11, Paragraph 3.B.(2).

4. Prepare the laminating resin (Material No. 13EBC1), refer to Chapter 51−77−11, Paragraph 

6.B.(2) and 4.A.(3).

5. Prepare the repair plies (MIL−C−9084C TYPE VIIIA or B − style 7781 dry glass fabric), refer to

Chapter 51−77−11, Paragraph 4.H. For ply dimensions and orientation refer to Figure 1.

NOTE: Round all corners with radii 12mm (0.5 in.) minimum.

6. Prepare the laminating resin, refer to Chapter 51−77−11, Paragraph 6.B.(2) and 4.A.(3).

7. Apply repair plies to the repair area as shown in Figure 1, refer to Chapter 51−77−11, 

Paragraph 5.A.

8. If the repair cure shall be accelerated by heat:

− Install the vaccum bag, refer to Chapter 51−77−11, Paragraph 5.D.(1), respect modificatons

shown on Figure 2 and the heating equipment.

− Allow repair to cure under vacuum pressure, refer to Chapter 51−77−11, Paragraph 5.E.,

use 22 in. of hg (560 mm of hg or 75 Kpa) minimum. Let the resin gel for one hour at room

temperature, then cure for 4 hours at 60 C, refer to Chapter 51−77−11, Paragraph 5.E.

− Remove the vacuum bag and the heating equipment.

− Continue with step 10.

9. If the repair cure shall be performed at room temperature:

− Install the vacuum bag, refer to Chapter 51−77−11, Paragraph 5.D.(1) and respect modifications

shown on Figure 2.

− Allow repair to cure under vacuum pressure, refer to Chapter 51−77−11, Paragraph 5.E.,

use 22 in. of hg (560 mm of hg or 75 Kpa) minimum. Let the resin cure for six hours at room

temperature or perform resin gelation test outside the repair area, after resin gelation perform

cure for two hours (the latter approach must be applied if RT is below 18 C (65 F)).

− Remove the vacuum bag and continue with step 10 during the next stop.

10. Remove the flash tape. Ensure that the glass ply is correctly located and cured, refer to

Chapter 51−77−10, Paragraph 5.

11. Remove any resin remnants from the border area of the glass ply, use abrasive paper. Start with

280 grade and finish with 400 grade.

WARNING: CLEANING AGENT (MATERIAL NO. 08BBF1 or 08BBU9) IS DANGEROUS.

12. Clean the repair area with cleaning agent (Material No. 08BBF1 or 08BBU9), refer to Chapter 51−

77−10, Paragraph 4.E.(1)(a).

13. Restore the surface protection, refer to Chapter 51−75−12.

F_SB_555007_6_AAAA_01_03

Figure A-GAAAA - Sheet 01

Closing of ventilation holes

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 88

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

Figure 1 − Ply lay−up

Ply 2 0/90 42 x 42mm

Ply 1 45 30 x 30mm

Ply 3 45 54 x 54mm

NON PERFORATING GLASS PLY FLASH TAPE

PARTING FILM

RUBBER CAUL

PLATE

BREATHER

DRY GLASS FABRIC

OR PEEL PLY

VACUUM GAGE VACUUM SOURCE

VACUUM BAG FILM

VACCUM BAG

SEALANT TAPE

NOTE:

01 RUBBER CAUL PLATE IS MANDATORY, 

01

REFER TO CHAPTER 51−77−11, PARAGRAPH 3.C.

Figure 2 − Bagging for curing process

F_SB_555007_6_AAAA_02_00

Figure A-GAAAA - Sheet 02

Closing of ventilation holes

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 89

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

PAINT THICKNESS MEASUREMENT USING THE PAINT BORER ON THE RUDDER SIDE SHELL

THE PAINT THICKNESS MUST BE DETERMINED FOR A CORRECT SETTING OF THE

PULSE THERMOGRAPHY INSPECTION PARAMETERS. IF THE THICKNESS IS UNKNOWN

DETERMINE THE THICKNESS WITH THE PAINT BORER.

DESCRIPTION

1. GENERAL

A. THIS PROCEDURE CONTAINS THE INSPECTION PROCEDURE DESCRIBING

PAINT THICKNESS MEASUREMENT USING THE PAINT BORER ON

THE RUDDER SIDE SHELL.

PROCEDURE

1 TASK SUPPORTING DATA

A. AREA OF APPLICABILITY

ALL RUDDER INSPECTED WITH NTM 55−40−50

B. DESCRIPTION OF POSSIBLE DAMAGE

THE PAINT THICKNESS MUST BE DETERMINED FOR A CORRECT SETTING OF THE

PULSE THERMOGRAPHY INSPECTION PARAMETERS. IF THE THICKNESS IS UNKNOWN

DETERMINE THE THICKNESS WITH THE PAINT BORER.

C. JOB SETUP INFORMATION

(1) TOOLING

PREFERRED TOOL: PAINT BORER 518MC WITH THE DRILLS IN TABLE 1

ALTERNATIVE TOOL: PAINT BORER 518 OR PAINT BORER 518S WITH THE DRILLS

 IN TABLE 1

ADDITIONAL DOCUMENT: OPERATING MANUAL PAINT BORER

TABLE 1 : DRILLS

F_SB_555007_6_ABAA_01_04

Figure A-GABAA - Sheet 01

Paint borer instructions

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 90

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

2 PROCEDURE:

1. PREPARE THE PAINT BORER ACCORDING TO THE OPERATING

1. PLACE THE PAINT BORER ON THE AREA, WHERE THE THICKNESS OF THE

 RUDDER PAINT HAS TO BE MEASURED, SEE FIG. A−GABAA SHEET 3+4

2. DO THE DRILLING AND THE PAINT THICKNESS MEASUREMENT ACCORDING 

 PAINT BORER OPERATING INSTRUCTIONS, REFER ALSO

 CAUTION: DO NOT DRILL DEEPLY INTO THE BASE MATERIAL (CFRP OR GFRP). ONLY A

TINY BASE MATERIAL SPOT IS ENOUGH TO MEASURE THE PAINT

THICKNESS, REFER TO FIG. A−GABAA SHEET 5+6

3. APPLY A CONTRAST MARK (WITH A NON PERMANENT MARKER PEN) ON THE

 THE SPOT OF MEASUREMENT. IF THE RUDDER PAINT IS LIGHT (E.G. YELLOW, 

 WHITE ...), USE A DARK (BLACK) PEN TO ENHANCE CONTRAST OF THE TOP

 COATING, IN CASE OF A DARK TOP COAT USE A LIGHT (WHITE) PEN. SEE

A. PREPARATION FOR INSPECTION

B. INSTRUMENT ADJUSTMENT

1. NO

C: INSPECTION PROCEDURE

 INSTRUCTIONS.

4. RECORD ALL THE MEASURED PAINT THICKNESS VALUES FOR THE

 PULSE THERMOGRAPHY INSPECTION.

5. AFTER MEASUREMENT SEAL THE SPOT WHERE DRILLED − REFER TO

 SRM 51−75−10.

 FIG. A−GABAA SHEET 7+8

 TO FIGURE A−GABAA SHEET 3−8

− IF THE LAYER THICKNESS IS NOT KNOWN,

INITIALLY USE A DRILL WITH 20−2000 m ( CUT ANGLE: 45°)

TO BRING THE FULL SECTION INTO VIEW;

CHANGE TO 10−1000 m (CUT ANGLE: 26.6°) IF THICKNESS

TURNS OUT TO BE 1000 m OR LESS

μ 

μ 

μ 

CAUTION: IT IS IMPORTANT TO HAVE THE ABOVE SPECIFIED DRILLS AVAILABLE.

CONTACT DRILL SUPPLIER IF THE CUTTING ANGLE AND DRILL NUMBERING

CAUTION: DO NOT USE ULTRASONIC OR EDDY CURRENT BASED PAINT THICKNESS

MEASUREMENT DEVICES, AS EDDY CURRENT ONLY WORKS ON METALLIC

AND FOR ULTRASONIC BASED DEVICES THE NUMBER OF POSSIBLE PAINT

LAYERS IS TOO HIGH TO GET RELIABLE RESULTS.

IS UNKNOWN.

F_SB_555007_6_ABAA_02_05

Figure A-GABAA - Sheet 02

Paint borer instructions

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 91

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

Z326

A

A

LH SHOWN

RH SIMILAR

C D E

B D E

CFRP

AREA

GFRP

AREA

F_SB_555007_6_ABAA_03_01

Figure A-GABAA - Sheet 03

Paint borer instructions

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 92

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

D E

PAINT SYSTEM

DIFFERENT LAYERS

(E.G. FILLER, PRIMER,

TOP COAT, ...)

CFRP

HONEYCOMB

CORE

d

NOTE:

01 DRILL HOLE

01

d = PAINT SYSTEM

THICKNESS

SPOT DRILLING

DETERMINATION OF

PAINT THICKNESS

PAINT SYSTEM

DIFFERENT LAYERS

(E.G. FILLER, PRIMER,

TOP COAT, ...)

GFRP

HONEYCOMB

CORE

d 01

B

C

F

G

F_SB_555007_6_ABAA_04_01

Figure A-GABAA - Sheet 04

Paint borer instructions

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 93

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

F

1) NOT DRILLED DEEP

ENOUGH

2) GOOD DRILLED DEPTH 

(TINY CFRP SPOT)

3) DRILLED TO DEEP

(BIG CFRP SPOT)

7) DRILLED TO DEEP

(DAMAGE OF THE HONEYCOMB

6) DRILLED TO DEEP

(BIG CFRP SPOT)

5) GOOD DRILLED

DEPTH (TINY

4) NOT DRILLED

DEEP ENOUGH

CFRP SPOT) CORE)

F_SB_555007_6_ABAA_05_00

Figure A-GABAA - Sheet 05

Paint borer instructions

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 94

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

8) NOT DRILLED DEEP

ENOUGH

9) NOT DRILLED DEEP

ENOUGH

10) GOOD DRILLED

DEPTH

11) DRILLED TOO DEEP

(BIG GFRP SPOT)

12) GOOD DRILLED DEPTH

(DAMAGE OF THE

13) DRILLED TOO DEEP

(TINY GFRP SPOT)

14) DRILLED TOO DEEP

(DAMAGE OF THE

(TINY GFRP SPOT)

HONEYCOMB CORE) HONEYCOMB CORE)

G

F_SB_555007_6_ABAA_06_00

Figure A-GABAA - Sheet 06

Paint borer instructions

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 95

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

F_SB_555007_6_ABAA_07_00

Figure A-GABAA - Sheet 07

Paint borer instructions

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 96

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

**CONF ALL

BR1

BR2

BR3

BR4

BR5

BR6

BR7

200.0mm (7.87in.) AFT OF BR7 RIVET CENTER

200.0mm (7.87in.) FWD OF HOIST POINT CENTER LINE

PROPOSAL:

1SPOT IN GFRP AREA

6SPOTS IN CFRP AREA

A

B

C

A

B

C

D

200.0mm (7.87in.) FWD OF HOIST POINT CENTER LINE

D

600.0mm (23.62in.)

600.0mm (23.62in.)

200.0mm (7.87in.) FROM

BR2 RIVET CENTER LINE

F_SB_555007_6_ABAA_08_02

Figure A-GABAA - Sheet 08

Paint borer instructions

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 97

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

REPORTING SHEET

TITLE: STABILIZERS - RUDDER SIDE SHELL SANDWICH REPAIR

INSPECTION

MODIFICATION No.: None

Please complete the appropriate item (A or B):

A - SB WILL BE embodied YES/NO (if NO please comment)

If YES, aircraft concerned (as per SB effectivity by default) and planned dates (month/year) of

embodiment:

B - SB HAS BEEN embodied on aircraft:

Operator comments:

From Airline:

Name/Title:

Signature: Date:

If operational documentation is affected (see Paragraph 1.K of this SB): If information is needed prior to

next normal revision or prior to SB embodiment, please indicate required service(s):

Either: Modification Operational Impact (MOI), if available YES/NO

Or : Intermediate revision YES/NO

Important Information: This SB will only be incorporated in your maintenance and operational

documentation if this sheet is returned to Airbus and signed by a duly authorised representative. With

the next feasible revision, this will result in

- Updating of maintenance documentation to show pre and post SB data.

- Updating of maintenance and operational documentation to show post SB data after embodiment.

If this SB requires previous or simultaneous accomplishment of other SBs, Airbus shall automatically

include them in the manual revisions. Refer to SIL 00-037 for detailed information.

Please return this completed sheet to:

AIRBUS

CUSTOMER SERVICES DIRECTORATE

1 Rond Point Maurice Bellonte

31707 BLAGNAC CEDEX FRANCE

Attn: SDC32 Technical Data and Documentation Services

FAX: (+33) 5 61 93 28 06

e-mail: sb.reporting@airbus.com

or via your Resident Customer Support Office.

Alternatively, SB lists via letters or fax are also accepted.

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 1

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.
@A340-500/600

SERVICE BULLETIN

QUALITY PERCEPTION FORM

Use this form to tell us what is your perception of the quality of this Service Bulletin. The reported data

that you provide us will be used to analyse areas of difficulties and to take corrective action to further

improve the quality of our Service Bulletins.

We thank you for the time you have taken in completing this form.

(Please rate on a scale of 1 to 4, with 4 being the highest score)

- Quality rating of this SB 4321

- Quality rating of the Accomplishment Instructions 4321

- Quality rating of the Illustrations 4321

- Is this SB easy to understand ? Y/N

If you have had difficulties in the accomplishment of this SB please quote below the area(s) and give a

short description of the issue.

Planning Material Instructions

X Effectivity X Kit content X Preparation

X Reason X List of Materials Operator Supplied X Mod/Inspection

X Manpower X Industry support X Test

X References X Re-identification X Close-Up

X Publication X Tooling X Illustrations

Comments:

Operator: Date:

Name/Title:

Please return this form to:

AIRBUS

CUSTOMER SERVICES DIRECTORATE

1 Rond Point Maurice Bellonte

31707 BLAGNAC CEDEX FRANCE

Attn : SEM4 Service Bulletins Management

FAX : (33) 5 61 93 42 51

Or via your Resident Customer Support Office.

DATE: Feb 07/13 SERVICE BULLETIN No.: A340-55-5007

REVISION No.: 01 - Aug 20/14 Page: 1

6

Printed in FRANCE © AIRBUS S.A.S. 2007. All rights reserved.